#------------------------------------------------------------------------------
#$Date: 2016-03-23 22:17:56 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179475 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/72/4337286.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4337286
loop_
_publ_author_name
'Scherf, Lavinia M.'
'Zeilinger, Michael'
'Fässler, Thomas F'
_publ_section_title
;
 Li18Na2Ge17-A Compound Demonstrating Cation Effects on Cluster Shapes and
 Crystal Packing in Ternary Zintl Phases.
;
_journal_issue                   4
_journal_name_full               'Inorganic chemistry'
_journal_page_first              2096
_journal_page_last               2101
_journal_paper_doi               10.1021/ic4027046
_journal_volume                  53
_journal_year                    2014
_chemical_formula_moiety         '(Ge12), (Ge4), (Ge), 18(Li), 2(Na)'
_chemical_formula_sum            'Ge17 Li18 Na2'
_chemical_formula_weight         1404.93
_chemical_name_common            'Lithium Sodium Germanide'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           157
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      157
_symmetry_space_group_name_Hall  'P 3 -2'
_symmetry_space_group_name_H-M   'P 3 1 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   17.0905(4)
_cell_length_b                   17.0905(4)
_cell_length_c                   8.0783(2)
_cell_measurement_reflns_used    9426
_cell_measurement_temperature    123(2)
_cell_measurement_theta_max      33.0649
_cell_measurement_theta_min      2.3834
_cell_volume                     2043.43(8)
_computing_cell_refinement
' SAINT Version 7.56a, Bruker AXS Inc., Madison, Wisconsin, USA, 2008.'
_computing_data_collection
; APEX suite of crystallographic sotfware. APEX 2 Version 2008.4,
Bruker AXS Inc., Madison, Wisconsin, USA, 2008.
;
_computing_data_reduction
' SAINT Version 7.56a, Bruker AXS Inc., Madison, Wisconsin, USA, 2008.'
_computing_molecular_graphics    'Diamond 3.2i (Crystal Impact, 2012)'
_computing_publication_material  'SHELX-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      123(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'phi- and omega-rotation'
_diffrn_radiation_monochromator  'MONTEL optic'
_diffrn_radiation_source         'rotating anode FR591'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0407
_diffrn_reflns_av_sigmaI/netI    0.0250
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            47961
_diffrn_reflns_theta_full        33.16
_diffrn_reflns_theta_max         33.16
_diffrn_reflns_theta_min         2.38
_exptl_absorpt_coefficient_mu    18.459
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.3614
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS, Bruker, 2008b'
_exptl_crystal_colour            'metallic black'
_exptl_crystal_density_diffrn    3.425
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1860
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.11
_refine_diff_density_max         0.878
_refine_diff_density_min         -0.994
_refine_diff_density_rms         0.120
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.007(18)
_refine_ls_extinction_coef       0.00028(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_matrix_type           full
_refine_ls_number_parameters     191
_refine_ls_number_reflns         5466
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.0212
_refine_ls_R_factor_gt           0.0185
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0159P)²+0.9509P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0412
_refine_ls_wR_factor_ref         0.0420
_reflns_number_gt                5150
_reflns_number_total             5466
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic4027046_si_002.cif
_cod_data_source_block           Li18Na2Ge17
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      P31m
_cod_database_code               4337286
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ge1 Ge 0.339398(19) 0.0000 0.20480(5) 0.00955(7) Uani 1 2 d S
Ge2 Ge 0.580559(17) 0.246415(17) 0.97870(4) 0.01008(5) Uani 1 1 d .
Ge3 Ge 0.6667 0.3333 0.23971(5) 0.00961(9) Uani 1 3 d S
Ge4 Ge 0.08722(2) 0.0000 0.02877(6) 0.00946(7) Uani 1 2 d S
Ge5 Ge 0.0000 0.0000 0.76979(8) 0.00921(11) Uani 1 6 d S
Ge6 Ge 0.239875(16) 0.155814(15) 0.48856(3) 0.00770(5) Uani 1 1 d .
Ge7 Ge 0.419509(16) 0.243707(16) 0.49600(3) 0.00840(5) Uani 1 1 d .
Ge8 Ge 0.503328(15) 0.412291(16) 0.49809(3) 0.00829(5) Uani 1 1 d .
Ge9 Ge 0.328033(14) 0.152558(16) 0.74800(3) 0.00843(5) Uani 1 1 d .
Ge10 Ge 0.49594(2) 0.0000 0.74910(4) 0.00931(6) Uani 1 2 d S
Ge11 Ge 0.41729(2) 0.41729(2) 0.99578(4) 0.00884(6) Uani 1 2 d S
Ge12 Ge 0.329968(14) 0.242165(17) 0.99415(3) 0.00868(5) Uani 1 1 d .
Na1 Na 0.34615(10) 0.0000 0.5607(2) 0.0266(4) Uani 1 2 d S
Na2 Na 0.6667 0.3333 0.6086(3) 0.0431(7) Uani 1 3 d S
Na3 Na 0.0000 0.0000 0.3960(3) 0.0285(6) Uani 1 6 d S
Li1 Li 0.3291(3) 0.3291(3) 0.6799(9) 0.0166(15) Uani 1 2 d S
Li2 Li 0.3333(3) 0.3333(3) 0.3162(10) 0.0150(14) Uani 1 2 d S
Li3 Li 0.1651(4) 0.1651(4) 0.8062(9) 0.0153(12) Uani 1 2 d S
Li4 Li 0.4944(3) 0.3294(3) 0.8091(7) 0.0156(10) Uani 1 1 d .
Li5 Li 0.1726(4) 0.1726(4) 0.1776(9) 0.0157(12) Uani 1 2 d S
Li6 Li 0.4855(3) 0.0000 0.2409(8) 0.0129(11) Uani 1 2 d S
Li7 Li 0.1897(4) 0.0000 0.3152(8) 0.0186(13) Uani 1 2 d S
Li8 Li 0.1556(4) 0.0000 0.6740(8) 0.0160(12) Uani 1 2 d S
Li9 Li 0.2423(4) 0.0000 0.9634(9) 0.0181(13) Uani 1 2 d S
Li10 Li 0.4987(3) 0.1619(4) 0.3216(7) 0.0184(10) Uani 1 1 d .
Li11 Li 0.3382(3) 0.1476(3) 0.2332(6) 0.0140(9) Uani 1 1 d .
Li12 Li 0.5013(3) 0.3324(3) 0.1786(7) 0.0173(10) Uani 1 1 d .
Li13 Li 0.4331(3) 0.0943(3) 0.9449(7) 0.0190(10) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Li6 Ge1 Li11 119.35(9) . 5
Li6 Ge1 Li11 119.35(9) . .
Li11 Ge1 Li11 118.39(17) 5 .
Li6 Ge1 Li9 137.1(2) . 1_554
Li11 Ge1 Li9 75.06(12) 5 1_554
Li11 Ge1 Li9 75.06(12) . 1_554
Li6 Ge1 Li13 78.08(16) . 5_554
Li11 Ge1 Li13 76.69(14) 5 5_554
Li11 Ge1 Li13 132.60(16) . 5_554
Li9 Ge1 Li13 65.79(18) 1_554 5_554
Li6 Ge1 Li13 78.08(16) . 1_554
Li11 Ge1 Li13 132.60(16) 5 1_554
Li11 Ge1 Li13 76.69(14) . 1_554
Li9 Ge1 Li13 65.79(18) 1_554 1_554
Li13 Ge1 Li13 63.7(2) 5_554 1_554
Li6 Ge1 Li7 154.1(2) . .
Li11 Ge1 Li7 59.62(9) 5 .
Li11 Ge1 Li7 59.62(9) . .
Li9 Ge1 Li7 68.8(2) 1_554 .
Li13 Ge1 Li7 123.05(15) 5_554 .
Li13 Ge1 Li7 123.05(15) 1_554 .
Li6 Ge1 Na1 81.03(15) . .
Li11 Ge1 Na1 85.99(11) 5 .
Li11 Ge1 Na1 85.99(11) . .
Li9 Ge1 Na1 141.91(15) 1_554 .
Li13 Ge1 Na1 141.39(11) 5_554 .
Li13 Ge1 Na1 141.39(11) 1_554 .
Li7 Ge1 Na1 73.08(15) . .
Li6 Ge1 Li10 60.29(9) . 5
Li11 Ge1 Li10 59.59(12) 5 5
Li11 Ge1 Li10 155.83(16) . 5
Li9 Ge1 Li10 123.11(10) 1_554 5
Li13 Ge1 Li10 71.54(16) 5_554 5
Li13 Ge1 Li10 123.74(14) 1_554 5
Li7 Ge1 Li10 109.17(12) . 5
Na1 Ge1 Li10 69.93(12) . 5
Li6 Ge1 Li10 60.29(9) . .
Li11 Ge1 Li10 155.83(16) 5 .
Li11 Ge1 Li10 59.59(12) . .
Li9 Ge1 Li10 123.11(10) 1_554 .
Li13 Ge1 Li10 123.74(14) 5_554 .
Li13 Ge1 Li10 71.54(16) 1_554 .
Li7 Ge1 Li10 109.17(12) . .
Na1 Ge1 Li10 69.93(12) . .
Li10 Ge1 Li10 111.33(18) 5 .
Ge2 Ge2 Ge2 60.0 3_665 2_655
Ge2 Ge2 Ge3 60.183(7) 3_665 1_556
Ge2 Ge2 Ge3 60.185(7) 2_655 1_556
Ge2 Ge2 Li13 150.49(10) 3_665 .
Ge2 Ge2 Li13 148.40(10) 2_655 .
Ge3 Ge2 Li13 131.11(12) 1_556 .
Ge2 Ge2 Li4 64.11(9) 3_665 .
Ge2 Ge2 Li4 116.15(9) 2_655 .
Ge3 Ge2 Li4 113.22(10) 1_556 .
Li13 Ge2 Li4 87.88(14) . .
Ge2 Ge2 Li4 115.10(9) 3_665 2_655
Ge2 Ge2 Li4 62.89(8) 2_655 2_655
Ge3 Ge2 Li4 112.23(9) 1_556 2_655
Li13 Ge2 Li4 87.22(13) . 2_655
Li4 Ge2 Li4 123.0(2) . 2_655
Ge2 Ge2 Li12 113.49(9) 3_665 2_656
Ge2 Ge2 Li12 64.23(9) 2_655 2_656
Ge3 Ge2 Li12 62.35(11) 1_556 2_656
Li13 Ge2 Li12 93.66(14) . 2_656
Li4 Ge2 Li12 175.04(16) . 2_656
Li4 Ge2 Li12 61.87(15) 2_655 2_656
Ge2 Ge2 Li12 63.90(9) 3_665 1_556
Ge2 Ge2 Li12 113.22(10) 2_655 1_556
Ge3 Ge2 Li12 62.22(11) 1_556 1_556
Li13 Ge2 Li12 95.74(13) . 1_556
Li4 Ge2 Li12 62.12(15) . 1_556
Li4 Ge2 Li12 174.32(15) 2_655 1_556
Li12 Ge2 Li12 113.0(2) 2_656 1_556
Ge2 Ge2 Li10 113.57(10) 3_665 1_556
Ge2 Ge2 Li10 113.03(9) 2_655 1_556
Ge3 Ge2 Li10 62.22(10) 1_556 1_556
Li13 Ge2 Li10 68.90(16) . 1_556
Li4 Ge2 Li10 115.68(13) . 1_556
Li4 Ge2 Li10 115.04(13) 2_655 1_556
Li12 Ge2 Li10 60.74(13) 2_656 1_556
Li12 Ge2 Li10 61.92(12) 1_556 1_556
Ge2 Ge2 Na2 67.423(15) 3_665 .
Ge2 Ge2 Na2 67.422(15) 2_655 .
Ge3 Ge2 Na2 118.64(2) 1_556 .
Li13 Ge2 Na2 110.23(12) . .
Li4 Ge2 Na2 64.59(10) . .
Li4 Ge2 Na2 64.30(10) 2_655 .
Li12 Ge2 Na2 119.06(10) 2_656 .
Li12 Ge2 Na2 118.81(10) 1_556 .
Li10 Ge2 Na2 179.01(10) 1_556 .
Ge2 Ge3 Ge2 59.633(13) 2_654 1_554
Ge2 Ge3 Ge2 59.633(13) 2_654 3_664
Ge2 Ge3 Ge2 59.633(13) 1_554 3_664
Ge2 Ge3 Li12 115.10(12) 2_654 .
Ge2 Ge3 Li12 65.01(11) 1_554 .
Ge2 Ge3 Li12 64.80(11) 3_664 .
Ge2 Ge3 Li12 64.80(11) 2_654 3_665
Ge2 Ge3 Li12 115.10(12) 1_554 3_665
Ge2 Ge3 Li12 65.01(11) 3_664 3_665
Li12 Ge3 Li12 117.08(7) . 3_665
Ge2 Ge3 Li12 65.01(11) 2_654 2_655
Ge2 Ge3 Li12 64.80(11) 1_554 2_655
Ge2 Ge3 Li12 115.10(12) 3_664 2_655
Li12 Ge3 Li12 117.08(7) . 2_655
Li12 Ge3 Li12 117.08(7) 3_665 2_655
Ge2 Ge3 Li10 117.22(10) 2_654 .
Ge2 Ge3 Li10 67.80(11) 1_554 .
Ge2 Ge3 Li10 117.79(10) 3_664 .
Li12 Ge3 Li10 64.44(11) . .
Li12 Ge3 Li10 177.02(18) 3_665 .
Li12 Ge3 Li10 63.12(11) 2_655 .
Ge2 Ge3 Li10 67.80(11) 2_654 2_655
Ge2 Ge3 Li10 117.79(10) 1_554 2_655
Ge2 Ge3 Li10 117.22(10) 3_664 2_655
Li12 Ge3 Li10 177.02(18) . 2_655
Li12 Ge3 Li10 63.12(11) 3_665 2_655
Li12 Ge3 Li10 64.44(11) 2_655 2_655
Li10 Ge3 Li10 115.21(8) . 2_655
Ge2 Ge3 Li10 117.79(10) 2_654 3_665
Ge2 Ge3 Li10 117.22(10) 1_554 3_665
Ge2 Ge3 Li10 67.80(11) 3_664 3_665
Li12 Ge3 Li10 63.12(11) . 3_665
Li12 Ge3 Li10 64.44(11) 3_665 3_665
Li12 Ge3 Li10 177.02(18) 2_655 3_665
Li10 Ge3 Li10 115.21(8) . 3_665
Li10 Ge3 Li10 115.21(8) 2_655 3_665
Ge2 Ge3 Na2 144.960(8) 2_654 .
Ge2 Ge3 Na2 144.960(8) 1_554 .
Ge2 Ge3 Na2 144.960(8) 3_664 .
Li12 Ge3 Na2 99.94(12) . .
Li12 Ge3 Na2 99.94(12) 3_665 .
Li12 Ge3 Na2 99.94(12) 2_655 .
Li10 Ge3 Na2 77.16(11) . .
Li10 Ge3 Na2 77.16(11) 2_655 .
Li10 Ge3 Na2 77.16(11) 3_665 .
Ge5 Ge4 Ge4 59.833(9) 1_554 3
Ge5 Ge4 Ge4 59.833(9) 1_554 2
Ge4 Ge4 Ge4 60.0 3 2
Ge5 Ge4 Li9 114.20(15) 1_554 1_554
Ge4 Ge4 Li9 148.14(5) 3 1_554
Ge4 Ge4 Li9 148.14(5) 2 1_554
Ge5 Ge4 Li5 110.10(10) 1_554 .
Ge4 Ge4 Li5 116.58(8) 3 .
Ge4 Ge4 Li5 62.79(6) 2 .
Li9 Ge4 Li5 95.09(10) 1_554 .
Ge5 Ge4 Li5 110.10(10) 1_554 3
Ge4 Ge4 Li5 62.79(6) 3 3
Ge4 Ge4 Li5 116.58(8) 2 3
Li9 Ge4 Li5 95.09(10) 1_554 3
Li5 Ge4 Li5 129.6(3) . 3
Ge5 Ge4 Li7 178.33(13) 1_554 .
Ge4 Ge4 Li7 121.52(10) 3 .
Ge4 Ge4 Li7 121.52(10) 2 .
Li9 Ge4 Li7 64.13(19) 1_554 .
Li5 Ge4 Li7 70.35(11) . .
Li5 Ge4 Li7 70.35(11) 3 .
Ge5 Ge4 Li3 60.15(12) 1_554 3_554
Ge4 Ge4 Li3 64.83(5) 3 3_554
Ge4 Ge4 Li3 112.33(8) 2 3_554
Li9 Ge4 Li3 84.83(10) 1_554 3_554
Li5 Ge4 Li3 168.72(18) . 3_554
Li5 Ge4 Li3 61.56(18) 3 3_554
Li7 Ge4 Li3 119.21(13) . 3_554
Ge5 Ge4 Li3 60.15(12) 1_554 1_554
Ge4 Ge4 Li3 112.33(8) 3 1_554
Ge4 Ge4 Li3 64.83(5) 2 1_554
Li9 Ge4 Li3 84.83(10) 1_554 1_554
Li5 Ge4 Li3 61.56(18) . 1_554
Li5 Ge4 Li3 168.72(18) 3 1_554
Li7 Ge4 Li3 119.21(13) . 1_554
Li3 Ge4 Li3 107.3(2) 3_554 1_554
Ge5 Ge4 Li8 57.66(11) 1_554 1_554
Ge4 Ge4 Li8 109.09(10) 3 1_554
Ge4 Ge4 Li8 109.09(10) 2 1_554
Li9 Ge4 Li8 56.54(19) 1_554 1_554
Li5 Ge4 Li8 113.36(14) . 1_554
Li5 Ge4 Li8 113.36(14) 3 1_554
Li7 Ge4 Li8 120.67(17) . 1_554
Li3 Ge4 Li8 57.41(11) 3_554 1_554
Li3 Ge4 Li8 57.41(11) 1_554 1_554
Ge5 Ge4 Na3 117.85(2) 1_554 .
Ge4 Ge4 Na3 67.118(18) 3 .
Ge4 Ge4 Na3 67.118(18) 2 .
Li9 Ge4 Na3 127.94(15) 1_554 .
Li5 Ge4 Na3 67.47(13) . .
Li5 Ge4 Na3 67.47(13) 3 .
Li7 Ge4 Na3 63.81(13) . .
Li3 Ge4 Na3 121.17(9) 3_554 .
Li3 Ge4 Na3 121.17(9) 1_554 .
Li8 Ge4 Na3 175.51(12) 1_554 .
Ge4 Ge5 Ge4 60.335(17) 2_556 1_556
Ge4 Ge5 Ge4 60.335(17) 2_556 3_556
Ge4 Ge5 Ge4 60.335(17) 1_556 3_556
Ge4 Ge5 Li8 120.40(10) 2_556 .
Ge4 Ge5 Li8 70.75(13) 1_556 .
Ge4 Ge5 Li8 120.40(10) 3_556 .
Ge4 Ge5 Li8 120.40(10) 2_556 3
Ge4 Ge5 Li8 120.40(10) 1_556 3
Ge4 Ge5 Li8 70.75(13) 3_556 3
Li8 Ge5 Li8 112.52(11) . 3
Ge4 Ge5 Li8 70.75(13) 2_556 2
Ge4 Ge5 Li8 120.40(10) 1_556 2
Ge4 Ge5 Li8 120.40(10) 3_556 2
Li8 Ge5 Li8 112.52(11) . 2
Li8 Ge5 Li8 112.52(11) 3 2
Ge4 Ge5 Li3 68.10(12) 2_556 .
Ge4 Ge5 Li3 68.10(12) 1_556 .
Ge4 Ge5 Li3 119.52(14) 3_556 .
Li8 Ge5 Li3 63.35(6) . .
Li8 Ge5 Li3 169.7(2) 3 .
Li8 Ge5 Li3 63.35(6) 2 .
Ge4 Ge5 Li3 68.10(12) 2_556 2
Ge4 Ge5 Li3 119.52(14) 1_556 2
Ge4 Ge5 Li3 68.10(12) 3_556 2
Li8 Ge5 Li3 169.7(2) . 2
Li8 Ge5 Li3 63.35(6) 3 2
Li8 Ge5 Li3 63.35(6) 2 2
Li3 Ge5 Li3 118.94(5) . 2
Ge4 Ge5 Li3 119.52(14) 2_556 3
Ge4 Ge5 Li3 68.10(12) 1_556 3
Ge4 Ge5 Li3 68.10(12) 3_556 3
Li8 Ge5 Li3 63.35(6) . 3
Li8 Ge5 Li3 63.35(6) 3 3
Li8 Ge5 Li3 169.7(2) 2 3
Li3 Ge5 Li3 118.94(5) . 3
Li3 Ge5 Li3 118.94(5) 2 3
Ge4 Ge5 Na3 144.530(11) 2_556 .
Ge4 Ge5 Na3 144.530(11) 1_556 .
Ge4 Ge5 Na3 144.530(11) 3_556 .
Li8 Ge5 Na3 73.78(13) . .
Li8 Ge5 Na3 73.78(13) 3 .
Li8 Ge5 Na3 73.78(13) 2 .
Li3 Ge5 Na3 95.95(14) . .
Li3 Ge5 Na3 95.95(14) 2 .
Li3 Ge5 Na3 95.95(14) 3 .
Ge6 Ge6 Ge9 121.385(8) 4 .
Ge6 Ge6 Ge7 120.700(6) 4 .
Ge9 Ge6 Ge7 58.388(9) . .
Ge6 Ge6 Li11 125.62(10) 4 .
Ge9 Ge6 Li11 103.40(10) . .
Ge7 Ge6 Li11 58.38(9) . .
Ge6 Ge6 Li7 124.81(15) 4 .
Ge9 Ge6 Li7 107.13(14) . .
Ge7 Ge6 Li7 105.80(14) . .
Li11 Ge6 Li7 57.36(15) . .
Ge6 Ge6 Li8 112.63(13) 4 .
Ge9 Ge6 Li8 64.44(12) . .
Ge7 Ge6 Li8 115.59(13) . .
Li11 Ge6 Li8 113.72(15) . .
Li7 Ge6 Li8 65.15(15) . .
Ge6 Ge6 Li5 63.98(6) 4 .
Ge9 Ge6 Li5 170.22(11) . .
Ge7 Ge6 Li5 112.02(12) . .
Li11 Ge6 Li5 67.93(13) . .
Li7 Ge6 Li5 72.53(16) . .
Li8 Ge6 Li5 122.51(17) . .
Ge6 Ge6 Li3 64.65(6) 4 .
Ge9 Ge6 Li3 64.17(8) . .
Ge7 Ge6 Li3 111.34(11) . .
Li11 Ge6 Li3 167.57(13) . .
Li7 Ge6 Li3 124.91(16) . .
Li8 Ge6 Li3 62.66(14) . .
Li5 Ge6 Li3 124.39(11) . .
Ge6 Ge6 Li2 65.27(5) 4 .
Ge9 Ge6 Li2 112.22(13) . .
Ge7 Ge6 Li2 63.58(8) . .
Li11 Ge6 Li2 70.48(14) . .
Li7 Ge6 Li2 119.97(19) . .
Li8 Ge6 Li2 174.87(18) . .
Li5 Ge6 Li2 61.34(18) . .
Li3 Ge6 Li2 112.58(15) . .
Ge6 Ge6 Li1 65.45(5) 4 .
Ge9 Ge6 Li1 65.84(10) . .
Ge7 Ge6 Li1 63.69(7) . .
Li11 Ge6 Li1 114.99(14) . .
Li7 Ge6 Li1 169.19(15) . .
Li8 Ge6 Li1 115.91(17) . .
Li5 Ge6 Li1 112.89(15) . .
Li3 Ge6 Li1 60.68(18) . .
Li2 Ge6 Li1 59.00(18) . .
Ge8 Ge7 Ge9 121.304(11) . .
Ge8 Ge7 Li11 123.25(11) . .
Ge9 Ge7 Li11 106.93(10) . .
Ge8 Ge7 Ge6 119.107(10) . .
Ge9 Ge7 Ge6 59.604(9) . .
Li11 Ge7 Ge6 61.74(9) . .
Ge8 Ge7 Li10 116.30(12) . .
Ge9 Ge7 Li10 113.63(12) . .
Li11 Ge7 Li10 60.68(14) . .
Ge6 Ge7 Li10 114.89(11) . .
Ge8 Ge7 Li4 63.55(8) . .
Ge9 Ge7 Li4 65.99(9) . .
Li11 Ge7 Li4 172.77(13) . .
Ge6 Ge7 Li4 113.62(10) . .
Li10 Ge7 Li4 119.91(15) . .
Ge8 Ge7 Li12 64.00(9) . .
Ge9 Ge7 Li12 171.85(10) . .
Li11 Ge7 Li12 65.43(14) . .
Ge6 Ge7 Li12 112.76(10) . .
Li10 Ge7 Li12 65.89(15) . .
Li4 Ge7 Li12 121.71(13) . .
Ge8 Ge7 Li2 63.63(12) . .
Ge9 Ge7 Li2 113.02(13) . .
Li11 Ge7 Li2 71.55(17) . .
Ge6 Ge7 Li2 63.36(11) . .
Li10 Ge7 Li2 120.22(19) . .
Li4 Ge7 Li2 112.00(16) . .
Li12 Ge7 Li2 62.69(16) . .
Ge8 Ge7 Li1 64.70(11) . .
Ge9 Ge7 Li1 66.17(12) . .
Li11 Ge7 Li1 117.80(15) . .
Ge6 Ge7 Li1 63.61(12) . .
Li10 Ge7 Li1 178.43(17) . .
Li4 Ge7 Li1 61.54(16) . .
Li12 Ge7 Li1 114.07(15) . .
Li2 Ge7 Li1 58.92(17) . .
Ge7 Ge8 Ge10 122.476(12) . 3_665
Ge7 Ge8 Li6 124.36(12) . 3_665
Ge10 Ge8 Li6 103.87(10) 3_665 3_665
Ge7 Ge8 Ge8 120.185(7) . 4
Ge10 Ge8 Ge8 58.237(7) 3_665 4
Li6 Ge8 Ge8 59.55(7) 3_665 4
Ge7 Ge8 Li10 118.06(11) . 3_665
Ge10 Ge8 Li10 111.73(12) 3_665 3_665
Li6 Ge8 Li10 60.63(14) 3_665 3_665
Ge8 Ge8 Li10 112.28(11) 4 3_665
Ge7 Ge8 Li4 64.86(9) . .
Ge10 Ge8 Li4 65.72(9) 3_665 .
Li6 Ge8 Li4 169.56(14) 3_665 .
Ge8 Ge8 Li4 112.57(10) 4 .
Li10 Ge8 Li4 121.34(15) 3_665 .
Ge7 Ge8 Li12 65.63(9) . .
Ge10 Ge8 Li12 169.95(10) 3_665 .
Li6 Ge8 Li12 66.14(14) 3_665 .
Ge8 Ge8 Li12 113.30(10) 4 .
Li10 Ge8 Li12 65.05(15) 3_665 .
Li4 Ge8 Li12 124.29(13) . .
Ge7 Ge8 Li2 66.31(8) . .
Ge10 Ge8 Li2 112.42(10) 3_665 .
Li6 Ge8 Li2 68.77(17) 3_665 .
Ge8 Ge8 Li2 62.48(6) 4 .
Li10 Ge8 Li2 118.5(2) 3_665 .
Li4 Ge8 Li2 114.88(17) . .
Li12 Ge8 Li2 63.93(16) . .
Ge7 Ge8 Li1 65.86(8) . .
Ge10 Ge8 Li1 66.29(13) 3_665 .
Li6 Ge8 Li1 115.25(12) 3_665 .
Ge8 Ge8 Li1 63.01(6) 4 .
Li10 Ge8 Li1 175.29(13) 3_665 .
Li4 Ge8 Li1 62.23(15) . .
Li12 Ge8 Li1 116.10(17) . .
Li2 Ge8 Li1 59.93(18) . .
Ge12 Ge9 Ge7 116.224(12) . .
Ge12 Ge9 Ge6 117.306(12) . .
Ge7 Ge9 Ge6 62.008(10) . .
Ge12 Ge9 Li9 85.31(11) . .
Ge7 Ge9 Li9 156.47(12) . .
Ge6 Ge9 Li9 118.23(12) . .
Ge12 Ge9 Li8 114.66(12) . .
Ge7 Ge9 Li8 115.20(12) . .
Ge6 Ge9 Li8 60.40(11) . .
Li9 Ge9 Li8 57.98(16) . .
Ge12 Ge9 Li13 87.33(10) . .
Ge7 Ge9 Li13 110.33(10) . .
Ge6 Ge9 Li13 155.30(10) . .
Li9 Ge9 Li13 58.59(18) . .
Li8 Ge9 Li13 109.40(14) . .
Ge12 Ge9 Li3 63.28(13) . .
Ge7 Ge9 Li3 113.26(12) . .
Ge6 Ge9 Li3 63.01(14) . .
Li9 Ge9 Li3 84.09(17) . .
Li8 Ge9 Li3 61.11(15) . .
Li13 Ge9 Li3 134.81(17) . .
Ge12 Ge9 Li4 62.15(10) . .
Ge7 Ge9 Li4 62.13(10) . .
Ge6 Ge9 Li4 112.43(10) . .
Li9 Ge9 Li4 128.26(15) . .
Li8 Ge9 Li4 170.73(13) . .
Li13 Ge9 Li4 79.52(13) . .
Li3 Ge9 Li4 110.99(16) . .
Ge12 Ge9 Li1 63.06(14) . .
Ge7 Ge9 Li1 63.71(12) . .
Ge6 Ge9 Li1 63.33(13) . .
Li9 Ge9 Li1 139.27(17) . .
Li8 Ge9 Li1 110.94(15) . .
Li13 Ge9 Li1 137.12(15) . .
Li3 Ge9 Li1 59.63(15) . .
Li4 Ge9 Li1 59.79(14) . .
Ge12 Ge9 Na1 155.42(4) . .
Ge7 Ge9 Na1 80.77(3) . .
Ge6 Ge9 Na1 85.90(3) . .
Li9 Ge9 Na1 75.85(12) . .
Li8 Ge9 Na1 68.20(11) . .
Li13 Ge9 Na1 69.47(10) . .
Li3 Ge9 Na1 128.66(12) . .
Li4 Ge9 Na1 118.62(10) . .
Li1 Ge9 Na1 140.63(14) . .
Ge11 Ge10 Ge8 116.818(14) 2_655 6_655
Ge11 Ge10 Ge8 116.818(14) 2_655 2_655
Ge8 Ge10 Ge8 63.525(13) 6_655 2_655
Ge11 Ge10 Li13 87.03(11) 2_655 .
Ge8 Ge10 Li13 155.36(11) 6_655 .
Ge8 Ge10 Li13 112.89(10) 2_655 .
Ge11 Ge10 Li13 87.03(11) 2_655 5
Ge8 Ge10 Li13 112.89(10) 6_655 5
Ge8 Ge10 Li13 155.36(11) 2_655 5
Li13 Ge10 Li13 59.2(2) . 5
Ge11 Ge10 Li4 63.18(10) 2_655 2_655
Ge8 Ge10 Li4 113.68(10) 6_655 2_655
Ge8 Ge10 Li4 61.90(10) 2_655 2_655
Li13 Ge10 Li4 81.61(14) . 2_655
Li13 Ge10 Li4 132.30(15) 5 2_655
Ge11 Ge10 Li4 63.18(10) 2_655 6_655
Ge8 Ge10 Li4 61.90(10) 6_655 6_655
Ge8 Ge10 Li4 113.68(10) 2_655 6_655
Li13 Ge10 Li4 132.29(15) . 6_655
Li13 Ge10 Li4 81.61(14) 5 6_655
Li4 Ge10 Li4 111.97(19) 2_655 6_655
Ge11 Ge10 Na1 157.39(4) 2_655 .
Ge8 Ge10 Na1 81.98(3) 6_655 .
Ge8 Ge10 Na1 81.98(3) 2_655 .
Li13 Ge10 Na1 73.40(11) . .
Li13 Ge10 Na1 73.40(11) 5 .
Li4 Ge10 Na1 122.93(10) 2_655 .
Li4 Ge10 Na1 122.93(10) 6_655 .
Ge11 Ge10 Li1 63.92(14) 2_655 2_655
Ge8 Ge10 Li1 63.32(11) 6_655 2_655
Ge8 Ge10 Li1 63.32(11) 2_655 2_655
Li13 Ge10 Li1 139.18(14) . 2_655
Li13 Ge10 Li1 139.18(14) 5 2_655
Li4 Ge10 Li1 60.31(10) 2_655 2_655
Li4 Ge10 Li1 60.31(10) 6_655 2_655
Na1 Ge10 Li1 138.68(15) . 2_655
Ge10 Ge11 Li6 103.36(13) 3_665 3_666
Ge10 Ge11 Ge12 120.829(14) 3_665 .
Li6 Ge11 Ge12 124.05(10) 3_666 .
Ge10 Ge11 Ge12 120.829(14) 3_665 4
Li6 Ge11 Ge12 124.04(10) 3_666 4
Ge12 Ge11 Ge12 60.181(12) . 4
Ge10 Ge11 Li4 66.29(9) 3_665 .
Li6 Ge11 Li4 115.02(11) 3_666 .
Ge12 Ge11 Li4 62.82(9) . .
Ge12 Ge11 Li4 113.33(9) 4 .
Ge10 Ge11 Li4 66.29(9) 3_665 4
Li6 Ge11 Li4 115.02(11) 3_666 4
Ge12 Ge11 Li4 113.33(9) . 4
Ge12 Ge11 Li4 62.82(9) 4 4
Li4 Ge11 Li4 116.5(2) . 4
Ge10 Ge11 Li12 114.18(11) 3_665 4_556
Li6 Ge11 Li12 67.17(11) 3_666 4_556
Ge12 Ge11 Li12 115.59(10) . 4_556
Ge12 Ge11 Li12 64.44(9) 4 4_556
Li4 Ge11 Li12 177.72(14) . 4_556
Li4 Ge11 Li12 62.28(15) 4 4_556
Ge10 Ge11 Li12 114.18(11) 3_665 1_556
Li6 Ge11 Li12 67.17(11) 3_666 1_556
Ge12 Ge11 Li12 64.45(9) . 1_556
Ge12 Ge11 Li12 115.59(10) 4 1_556
Li4 Ge11 Li12 62.28(15) . 1_556
Li4 Ge11 Li12 177.72(14) 4 1_556
Li12 Ge11 Li12 118.9(2) 4_556 1_556
Ge10 Ge11 Li2 172.36(13) 3_665 1_556
Li6 Ge11 Li2 69.00(18) 3_666 1_556
Ge12 Ge11 Li2 65.47(11) . 1_556
Ge12 Ge11 Li2 65.47(11) 4 1_556
Li4 Ge11 Li2 116.34(10) . 1_556
Li4 Ge11 Li2 116.34(10) 4 1_556
Li12 Ge11 Li2 63.51(12) 4_556 1_556
Li12 Ge11 Li2 63.51(12) 1_556 1_556
Ge10 Ge11 Li1 67.24(12) 3_665 .
Li6 Ge11 Li1 170.60(18) 3_666 .
Ge12 Ge11 Li1 63.61(10) . .
Ge12 Ge11 Li1 63.61(10) 4 .
Li4 Ge11 Li1 62.07(11) . .
Li4 Ge11 Li1 62.07(11) 4 .
Li12 Ge11 Li1 115.88(11) 4_556 .
Li12 Ge11 Li1 115.88(11) 1_556 .
Li2 Ge11 Li1 120.41(17) 1_556 .
Ge9 Ge12 Li11 101.57(10) . 1_556
Ge9 Ge12 Ge11 122.343(13) . .
Li11 Ge12 Ge11 122.84(10) 1_556 .
Ge9 Ge12 Ge12 121.269(8) . 4
Li11 Ge12 Ge12 126.36(10) 1_556 4
Ge11 Ge12 Ge12 59.910(6) . 4
Ge9 Ge12 Li5 116.79(13) . 1_556
Li11 Ge12 Li5 70.95(13) 1_556 1_556
Ge11 Ge12 Li5 111.63(9) . 1_556
Ge12 Ge12 Li5 61.97(6) 4 1_556
Ge9 Ge12 Li4 67.17(9) . .
Li11 Ge12 Li4 111.90(13) 1_556 .
Ge11 Ge12 Li4 63.37(9) . .
Ge12 Ge12 Li4 113.56(9) 4 .
Li5 Ge12 Li4 174.96(12) 1_556 .
Ge9 Ge12 Li3 65.77(9) . .
Li11 Ge12 Li3 117.29(14) 1_556 .
Ge11 Ge12 Li3 113.45(8) . .
Ge12 Ge12 Li3 63.13(6) 4 .
Li5 Ge12 Li3 64.31(19) 1_556 .
Li4 Ge12 Li3 116.45(19) . .
Ge9 Ge12 Li12 115.39(11) . 1_556
Li11 Ge12 Li12 66.16(13) 1_556 1_556
Ge11 Ge12 Li12 62.91(9) . 1_556
Ge12 Ge12 Li12 114.07(9) 4 1_556
Li5 Ge12 Li12 116.9(2) 1_556 1_556
Li4 Ge12 Li12 61.96(15) . 1_556
Li3 Ge12 Li12 176.33(13) . 1_556
Ge9 Ge12 Li1 67.76(9) . .
Li11 Ge12 Li1 169.05(13) 1_556 .
Ge11 Ge12 Li1 64.35(12) . .
Ge12 Ge12 Li1 63.81(6) 4 .
Li5 Ge12 Li1 115.45(12) 1_556 .
Li4 Ge12 Li1 62.46(13) . .
Li3 Ge12 Li1 61.62(18) . .
Li12 Ge12 Li1 115.27(15) 1_556 .
Ge9 Ge12 Li2 173.14(9) . 1_556
Li11 Ge12 Li2 71.57(14) 1_556 1_556
Ge11 Ge12 Li2 63.15(11) . 1_556
Ge12 Ge12 Li2 64.49(7) 4 1_556
Li5 Ge12 Li2 61.53(17) 1_556 1_556
Li4 Ge12 Li2 114.94(15) . 1_556
Li3 Ge12 Li2 116.93(13) . 1_556
Li12 Ge12 Li2 62.35(14) 1_556 1_556
Li1 Ge12 Li2 119.09(12) . 1_556
Ge1 Na1 Ge10 123.04(6) . .
Ge1 Na1 Ge9 117.25(4) . .
Ge10 Na1 Ge9 101.19(5) . .
Ge1 Na1 Ge9 117.25(4) . 5
Ge10 Na1 Ge9 101.19(5) . 5
Ge9 Na1 Ge9 91.18(5) . 5
Ge1 Na1 Li10 55.40(10) . 5
Ge10 Na1 Li10 88.90(9) . 5
Ge9 Na1 Li10 169.91(10) . 5
Ge9 Na1 Li10 87.17(8) 5 5
Ge1 Na1 Li10 55.40(10) . .
Ge10 Na1 Li10 88.90(9) . .
Ge9 Na1 Li10 87.17(8) . .
Ge9 Na1 Li10 169.91(10) 5 .
Li10 Na1 Li10 92.71(18) 5 .
Ge1 Na1 Li7 51.13(11) . .
Ge10 Na1 Li7 174.17(13) . .
Ge9 Na1 Li7 82.84(8) . .
Ge9 Na1 Li7 82.84(8) 5 .
Li10 Na1 Li7 87.08(13) 5 .
Li10 Na1 Li7 87.08(13) . .
Ge1 Na1 Li8 103.41(12) . .
Ge10 Na1 Li8 133.56(12) . .
Ge9 Na1 Li8 51.61(5) . .
Ge9 Na1 Li8 51.61(5) 5 .
Li10 Na1 Li8 120.88(10) 5 .
Li10 Na1 Li8 120.88(10) . .
Li7 Na1 Li8 52.28(15) . .
Ge1 Na1 Li13 154.36(9) . 5
Ge10 Na1 Li13 51.29(8) . 5
Ge9 Na1 Li13 87.65(10) . 5
Ge9 Na1 Li13 52.01(8) 5 5
Li10 Na1 Li13 99.11(13) 5 5
Li10 Na1 Li13 137.76(13) . 5
Li7 Na1 Li13 133.64(13) . 5
Li8 Na1 Li13 86.93(13) . 5
Ge1 Na1 Li13 154.36(9) . .
Ge10 Na1 Li13 51.29(8) . .
Ge9 Na1 Li13 52.01(8) . .
Ge9 Na1 Li13 87.65(10) 5 .
Li10 Na1 Li13 137.76(13) 5 .
Li10 Na1 Li13 99.11(13) . .
Li7 Na1 Li13 133.64(13) . .
Li8 Na1 Li13 86.93(13) . .
Li13 Na1 Li13 47.43(16) 5 .
Ge1 Na1 Li6 44.98(10) . .
Ge10 Na1 Li6 78.05(10) . .
Ge9 Na1 Li6 134.26(3) . .
Ge9 Na1 Li6 134.26(3) 5 .
Li10 Na1 Li6 47.24(9) 5 .
Li10 Na1 Li6 47.24(9) . .
Li7 Na1 Li6 96.11(15) . .
Li8 Na1 Li6 148.39(15) . .
Li13 Na1 Li6 121.65(12) 5 .
Li13 Na1 Li6 121.65(12) . .
Ge1 Na1 Li11 43.22(7) . 5
Ge10 Na1 Li11 133.57(7) . 5
Ge9 Na1 Li11 124.79(8) . 5
Ge9 Na1 Li11 74.23(8) 5 5
Li10 Na1 Li11 45.26(10) 5 5
Li10 Na1 Li11 98.59(13) . 5
Li7 Na1 Li11 43.24(8) . 5
Li8 Na1 Li11 80.23(11) . 5
Li13 Na1 Li11 118.39(11) 5 5
Li13 Na1 Li11 161.76(12) . 5
Li6 Na1 Li11 74.38(12) . 5
Ge3 Na2 Li4 119.09(9) . 2_655
Ge3 Na2 Li4 119.09(10) . 3_665
Li4 Na2 Li4 98.36(12) 2_655 3_665
Ge3 Na2 Li4 119.09(9) . .
Li4 Na2 Li4 98.36(12) 2_655 .
Li4 Na2 Li4 98.36(12) 3_665 .
Ge3 Na2 Ge2 153.684(18) . 2_655
Li4 Na2 Ge2 50.70(9) 2_655 2_655
Li4 Na2 Ge2 51.28(9) 3_665 2_655
Li4 Na2 Ge2 87.22(10) . 2_655
Ge3 Na2 Ge2 153.684(18) . 3_665
Li4 Na2 Ge2 87.22(10) 2_655 3_665
Li4 Na2 Ge2 50.70(9) 3_665 3_665
Li4 Na2 Ge2 51.28(9) . 3_665
Ge2 Na2 Ge2 45.15(3) 2_655 3_665
Ge3 Na2 Ge2 153.684(18) . .
Li4 Na2 Ge2 51.28(9) 2_655 .
Li4 Na2 Ge2 87.22(10) 3_665 .
Li4 Na2 Ge2 50.70(9) . .
Ge2 Na2 Ge2 45.15(3) 2_655 .
Ge2 Na2 Ge2 45.15(3) 3_665 .
Ge3 Na2 Li10 51.36(9) . .
Li4 Na2 Li10 87.93(11) 2_655 .
Li4 Na2 Li10 170.45(13) 3_665 .
Li4 Na2 Li10 87.75(11) . .
Ge2 Na2 Li10 136.89(9) 2_655 .
Ge2 Na2 Li10 137.36(8) 3_665 .
Ge2 Na2 Li10 102.33(9) . .
Ge3 Na2 Li10 51.36(9) . 2_655
Li4 Na2 Li10 87.75(11) 2_655 2_655
Li4 Na2 Li10 87.93(11) 3_665 2_655
Li4 Na2 Li10 170.45(13) . 2_655
Ge2 Na2 Li10 102.32(9) 2_655 2_655
Ge2 Na2 Li10 136.89(9) 3_665 2_655
Ge2 Na2 Li10 137.36(8) . 2_655
Li10 Na2 Li10 85.13(14) . 2_655
Ge3 Na2 Li10 51.36(9) . 3_665
Li4 Na2 Li10 170.45(13) 2_655 3_665
Li4 Na2 Li10 87.75(11) 3_665 3_665
Li4 Na2 Li10 87.93(11) . 3_665
Ge2 Na2 Li10 137.36(8) 2_655 3_665
Ge2 Na2 Li10 102.32(9) 3_665 3_665
Ge2 Na2 Li10 136.89(8) . 3_665
Li10 Na2 Li10 85.13(14) . 3_665
Li10 Na2 Li10 85.13(14) 2_655 3_665
Ge5 Na3 Li7 101.38(12) . 3
Ge5 Na3 Li7 101.38(12) . 2
Li7 Na3 Li7 116.20(8) 3 2
Ge5 Na3 Li7 101.38(12) . .
Li7 Na3 Li7 116.20(8) 3 .
Li7 Na3 Li7 116.20(8) 2 .
Ge5 Na3 Ge4 153.32(2) . .
Li7 Na3 Ge4 92.51(12) 3 .
Li7 Na3 Ge4 92.51(12) 2 .
Li7 Na3 Ge4 51.94(12) . .
Ge5 Na3 Ge4 153.32(2) . 3
Li7 Na3 Ge4 51.94(12) 3 3
Li7 Na3 Ge4 92.51(12) 2 3
Li7 Na3 Ge4 92.51(12) . 3
Ge4 Na3 Ge4 45.76(4) . 3
Ge5 Na3 Ge4 153.32(2) . 2
Li7 Na3 Ge4 92.51(12) 3 2
Li7 Na3 Ge4 51.94(12) 2 2
Li7 Na3 Ge4 92.51(12) . 2
Ge4 Na3 Ge4 45.76(4) . 2
Ge4 Na3 Ge4 45.77(4) 3 2
Ge5 Na3 Li5 120.88(12) . .
Li7 Na3 Li5 137.74(19) 3 .
Li7 Na3 Li5 58.54(6) 2 .
Li7 Na3 Li5 58.54(6) . .
Ge4 Na3 Li5 49.36(10) . .
Ge4 Na3 Li5 85.80(13) 3 .
Ge4 Na3 Li5 49.36(10) 2 .
Ge5 Na3 Li5 120.88(12) . 2
Li7 Na3 Li5 58.53(6) 3 2
Li7 Na3 Li5 58.54(6) 2 2
Li7 Na3 Li5 137.74(19) . 2
Ge4 Na3 Li5 85.80(13) . 2
Ge4 Na3 Li5 49.36(10) 3 2
Ge4 Na3 Li5 49.36(10) 2 2
Li5 Na3 Li5 96.02(16) . 2
Ge5 Na3 Li5 120.88(12) . 3
Li7 Na3 Li5 58.53(6) 3 3
Li7 Na3 Li5 137.74(19) 2 3
Li7 Na3 Li5 58.54(6) . 3
Ge4 Na3 Li5 49.36(10) . 3
Ge4 Na3 Li5 49.36(10) 3 3
Ge4 Na3 Li5 85.80(13) 2 3
Li5 Na3 Li5 96.02(16) . 3
Li5 Na3 Li5 96.02(16) 2 3
Ge5 Na3 Li8 49.82(11) . .
Li7 Na3 Li8 120.12(8) 3 .
Li7 Na3 Li8 120.12(8) 2 .
Li7 Na3 Li8 51.57(15) . .
Ge4 Na3 Li8 103.50(10) . .
Ge4 Na3 Li8 138.42(9) 3 .
Ge4 Na3 Li8 138.42(9) 2 .
Li5 Na3 Li8 90.19(11) . .
Li5 Na3 Li8 170.70(16) 2 .
Li5 Na3 Li8 90.19(11) 3 .
Ge5 Na3 Li8 49.82(11) . 2
Li7 Na3 Li8 120.12(8) 3 2
Li7 Na3 Li8 51.57(15) 2 2
Li7 Na3 Li8 120.12(8) . 2
Ge4 Na3 Li8 138.42(9) . 2
Ge4 Na3 Li8 138.42(9) 3 2
Ge4 Na3 Li8 103.50(10) 2 2
Li5 Na3 Li8 90.19(11) . 2
Li5 Na3 Li8 90.19(11) 2 2
Li5 Na3 Li8 170.70(16) 3 2
Li8 Na3 Li8 82.85(16) . 2
Li2 Li1 Ge12 150.21(14) . .
Li2 Li1 Ge12 150.21(14) . 4
Ge12 Li1 Ge12 52.38(13) . 4
Li2 Li1 Ge11 148.0(3) . .
Ge12 Li1 Ge11 52.04(13) . .
Ge12 Li1 Ge11 52.04(13) 4 .
Li2 Li1 Ge8 59.14(17) . 4
Ge12 Li1 Ge8 144.3(2) . 4
Ge12 Li1 Ge8 114.28(12) 4 4
Ge11 Li1 Ge8 92.81(16) . 4
Li2 Li1 Ge8 59.14(17) . .
Ge12 Li1 Ge8 114.28(12) . .
Ge12 Li1 Ge8 144.3(2) 4 .
Ge11 Li1 Ge8 92.81(16) . .
Ge8 Li1 Ge8 53.98(11) 4 .
Li2 Li1 Li3 111.4(3) . .
Ge12 Li1 Li3 58.04(16) . .
Ge12 Li1 Li3 58.04(16) 4 .
Ge11 Li1 Li3 100.6(2) . .
Ge8 Li1 Li3 149.95(12) 4 .
Ge8 Li1 Li3 149.95(12) . .
Li2 Li1 Ge6 60.15(17) . 4
Ge12 Li1 Ge6 116.20(19) . 4
Ge12 Li1 Ge6 94.29(13) 4 4
Ge11 Li1 Ge6 145.64(18) . 4
Ge8 Li1 Ge6 96.37(17) 4 4
Ge8 Li1 Ge6 119.2(3) . 4
Li3 Li1 Ge6 58.19(15) . 4
Li2 Li1 Ge6 60.15(17) . .
Ge12 Li1 Ge6 94.29(13) . .
Ge12 Li1 Ge6 116.20(19) 4 .
Ge11 Li1 Ge6 145.64(18) . .
Ge8 Li1 Ge6 119.2(3) 4 .
Ge8 Li1 Ge6 96.37(17) . .
Li3 Li1 Ge6 58.19(15) . .
Ge6 Li1 Ge6 49.10(11) 4 .
Li2 Li1 Ge7 60.26(13) . .
Ge12 Li1 Ge7 92.74(6) . .
Ge12 Li1 Ge7 144.51(18) 4 .
Ge11 Li1 Ge7 114.80(13) . .
Ge8 Li1 Ge7 97.93(19) 4 .
Ge8 Li1 Ge7 49.45(8) . .
Li3 Li1 Ge7 100.56(14) . .
Ge6 Li1 Ge7 96.64(19) 4 .
Ge6 Li1 Ge7 52.71(9) . .
Li2 Li1 Ge7 60.26(13) . 4
Ge12 Li1 Ge7 144.51(18) . 4
Ge12 Li1 Ge7 92.74(6) 4 4
Ge11 Li1 Ge7 114.80(13) . 4
Ge8 Li1 Ge7 49.45(8) 4 4
Ge8 Li1 Ge7 97.93(19) . 4
Li3 Li1 Ge7 100.56(14) . 4
Ge6 Li1 Ge7 52.71(9) 4 4
Ge6 Li1 Ge7 96.64(19) . 4
Ge7 Li1 Ge7 120.5(3) . 4
Li2 Li1 Li4 109.58(17) . .
Ge12 Li1 Li4 57.34(12) . .
Ge12 Li1 Li4 100.2(2) 4 .
Ge11 Li1 Li4 57.46(14) . .
Ge8 Li1 Li4 101.02(19) 4 .
Ge8 Li1 Li4 56.96(12) . .
Li3 Li1 Li4 108.87(18) . .
Ge6 Li1 Li4 150.28(18) 4 .
Ge6 Li1 Li4 101.20(10) . .
Ge7 Li1 Li4 57.36(10) . .
Ge7 Li1 Li4 150.4(2) 4 .
Ge8 Li2 Ge8 55.04(12) 4 .
Ge8 Li2 Li1 60.93(18) 4 .
Ge8 Li2 Li1 60.93(18) . .
Ge8 Li2 Ge11 94.98(16) 4 1_554
Ge8 Li2 Ge11 94.98(16) . 1_554
Li1 Li2 Ge11 152.4(3) . 1_554
Ge8 Li2 Li5 149.99(12) 4 .
Ge8 Li2 Li5 149.99(12) . .
Li1 Li2 Li5 110.8(3) . .
Ge11 Li2 Li5 96.8(2) 1_554 .
Ge8 Li2 Ge6 97.98(18) 4 4
Ge8 Li2 Ge6 121.7(3) . 4
Li1 Li2 Ge6 60.84(18) . 4
Ge11 Li2 Ge6 141.9(2) 1_554 4
Li5 Li2 Ge6 57.03(16) . 4
Ge8 Li2 Ge6 121.7(3) 4 .
Ge8 Li2 Ge6 97.98(18) . .
Li1 Li2 Ge6 60.84(18) . .
Ge11 Li2 Ge6 141.9(2) 1_554 .
Li5 Li2 Ge6 57.03(16) . .
Ge6 Li2 Ge6 49.45(10) 4 .
Ge8 Li2 Ge7 99.5(2) 4 .
Ge8 Li2 Ge7 50.06(8) . .
Li1 Li2 Ge7 60.82(14) . .
Ge11 Li2 Ge7 115.53(13) 1_554 .
Li5 Li2 Ge7 100.07(14) . .
Ge6 Li2 Ge7 97.4(2) 4 .
Ge6 Li2 Ge7 53.06(9) . .
Ge8 Li2 Ge7 50.06(8) 4 4
Ge8 Li2 Ge7 99.5(2) . 4
Li1 Li2 Ge7 60.82(14) . 4
Ge11 Li2 Ge7 115.53(13) 1_554 4
Li5 Li2 Ge7 100.07(14) . 4
Ge6 Li2 Ge7 53.06(9) 4 4
Ge6 Li2 Ge7 97.4(2) . 4
Ge7 Li2 Ge7 121.6(3) . 4
Ge8 Li2 Ge12 115.51(12) 4 4_554
Ge8 Li2 Ge12 146.0(2) . 4_554
Li1 Li2 Ge12 148.77(16) . 4_554
Ge11 Li2 Ge12 51.38(13) 1_554 4_554
Li5 Li2 Ge12 55.04(15) . 4_554
Ge6 Li2 Ge12 90.87(14) 4 4_554
Ge6 Li2 Ge12 112.1(2) . 4_554
Ge7 Li2 Ge12 142.5(2) . 4_554
Ge7 Li2 Ge12 92.38(7) 4 4_554
Ge8 Li2 Ge12 146.0(2) 4 1_554
Ge8 Li2 Ge12 115.51(12) . 1_554
Li1 Li2 Ge12 148.77(16) . 1_554
Ge11 Li2 Ge12 51.38(13) 1_554 1_554
Li5 Li2 Ge12 55.04(15) . 1_554
Ge6 Li2 Ge12 112.1(2) 4 1_554
Ge6 Li2 Ge12 90.87(14) . 1_554
Ge7 Li2 Ge12 92.38(7) . 1_554
Ge7 Li2 Ge12 142.5(2) 4 1_554
Ge12 Li2 Ge12 51.01(13) 4_554 1_554
Ge8 Li2 Li12 102.6(2) 4 .
Ge8 Li2 Li12 57.97(13) . .
Li1 Li2 Li12 111.81(18) . .
Ge11 Li2 Li12 57.35(13) 1_554 .
Li5 Li2 Li12 107.01(19) . .
Ge6 Li2 Li12 150.19(16) 4 .
Ge6 Li2 Li12 100.95(9) . .
Ge7 Li2 Li12 58.19(10) . .
Ge7 Li2 Li12 152.5(2) 4 .
Ge12 Li2 Li12 99.3(2) 4_554 .
Ge12 Li2 Li12 57.62(12) 1_554 .
Ge5 Li3 Ge12 140.33(19) . .
Ge5 Li3 Ge12 140.32(19) . 4
Ge12 Li3 Ge12 53.75(12) . 4
Ge5 Li3 Ge6 95.73(19) . .
Ge12 Li3 Ge6 97.73(14) . .
Ge12 Li3 Ge6 121.4(2) 4 .
Ge5 Li3 Ge6 95.73(19) . 4
Ge12 Li3 Ge6 121.4(2) . 4
Ge12 Li3 Ge6 97.73(14) 4 4
Ge6 Li3 Ge6 50.70(12) . 4
Ge5 Li3 Ge9 114.75(12) . .
Ge12 Li3 Ge9 50.96(7) . .
Ge12 Li3 Ge9 99.79(17) 4 .
Ge6 Li3 Ge9 52.81(8) . .
Ge6 Li3 Ge9 98.82(19) 4 .
Ge5 Li3 Ge9 114.75(12) . 4
Ge12 Li3 Ge9 99.78(17) . 4
Ge12 Li3 Ge9 50.95(7) 4 4
Ge6 Li3 Ge9 98.82(19) . 4
Ge6 Li3 Ge9 52.82(8) 4 4
Ge9 Li3 Ge9 124.5(2) . 4
Ge5 Li3 Li8 57.20(15) . .
Ge12 Li3 Li8 101.67(12) . .
Ge12 Li3 Li8 155.41(19) 4 .
Ge6 Li3 Li8 56.12(13) . .
Ge6 Li3 Li8 96.4(2) 4 .
Ge9 Li3 Li8 58.11(12) . .
Ge9 Li3 Li8 148.8(3) 4 .
Ge5 Li3 Li8 57.20(15) . 2
Ge12 Li3 Li8 155.41(19) . 2
Ge12 Li3 Li8 101.67(12) 4 2
Ge6 Li3 Li8 96.4(2) . 2
Ge6 Li3 Li8 56.12(13) 4 2
Ge9 Li3 Li8 148.8(3) . 2
Ge9 Li3 Li8 58.11(12) 4 2
Li8 Li3 Li8 102.9(3) . 2
Ge5 Li3 Li1 154.1(3) . .
Ge12 Li3 Li1 60.34(17) . .
Ge12 Li3 Li1 60.34(17) 4 .
Ge6 Li3 Li1 61.13(16) . .
Ge6 Li3 Li1 61.13(16) 4 .
Ge9 Li3 Li1 62.23(10) . .
Ge9 Li3 Li1 62.23(10) 4 .
Li8 Li3 Li1 110.63(19) . .
Li8 Li3 Li1 110.63(19) 2 .
Ge5 Li3 Li5 98.4(2) . 1_556
Ge12 Li3 Li5 56.08(16) . 1_556
Ge12 Li3 Li5 56.08(16) 4 1_556
Ge6 Li3 Li5 150.93(13) . 1_556
Ge6 Li3 Li5 150.93(13) 4 1_556
Ge9 Li3 Li5 98.13(16) . 1_556
Ge9 Li3 Li5 98.13(16) 4 1_556
Li8 Li3 Li5 112.56(19) . 1_556
Li8 Li3 Li5 112.56(19) 2 1_556
Li1 Li3 Li5 107.6(3) . 1_556
Ge5 Li3 Ge4 51.74(10) . 2_556
Ge12 Li3 Ge4 111.8(2) . 2_556
Ge12 Li3 Ge4 89.24(15) 4 2_556
Ge6 Li3 Ge4 146.8(2) . 2_556
Ge6 Li3 Ge4 118.20(12) 4 2_556
Ge9 Li3 Ge4 140.41(18) . 2_556
Ge9 Li3 Ge4 91.03(7) 4 2_556
Li8 Li3 Ge4 101.6(2) . 2_556
Li8 Li3 Ge4 62.31(14) 2 2_556
Li1 Li3 Ge4 147.74(16) . 2_556
Li5 Li3 Ge4 55.74(15) 1_556 2_556
Ge8 Li4 Ge2 139.21(19) . .
Ge8 Li4 Ge12 120.98(17) . .
Ge2 Li4 Ge12 96.13(14) . .
Ge8 Li4 Ge11 97.33(13) . .
Ge2 Li4 Ge11 119.58(18) . .
Ge12 Li4 Ge11 53.81(9) . .
Ge8 Li4 Ge7 51.60(9) . .
Ge2 Li4 Ge7 112.14(15) . .
Ge12 Li4 Ge7 97.06(14) . .
Ge11 Li4 Ge7 121.56(17) . .
Ge8 Li4 Ge2 111.46(15) . 3_665
Ge2 Li4 Ge2 53.00(9) . 3_665
Ge12 Li4 Ge2 120.11(18) . 3_665
Ge11 Li4 Ge2 94.66(14) . 3_665
Ge7 Li4 Ge2 139.66(19) . 3_665
Ge8 Li4 Ge10 52.38(8) . 3_665
Ge2 Li4 Ge10 143.24(18) . 3_665
Ge12 Li4 Ge10 99.05(14) . 3_665
Ge11 Li4 Ge10 50.54(7) . 3_665
Ge7 Li4 Ge10 98.99(15) . 3_665
Ge2 Li4 Ge10 90.60(12) 3_665 3_665
Ge8 Li4 Ge9 98.33(15) . .
Ge2 Li4 Ge9 92.47(12) . .
Ge12 Li4 Ge9 50.68(8) . .
Ge11 Li4 Ge9 99.38(14) . .
Ge7 Li4 Ge9 51.88(8) . .
Ge2 Li4 Ge9 145.05(17) 3_665 .
Ge10 Li4 Ge9 122.85(17) 3_665 .
Ge8 Li4 Li12 151.71(18) . 1_556
Ge2 Li4 Li12 60.21(14) . 1_556
Ge12 Li4 Li12 60.41(14) . 1_556
Ge11 Li4 Li12 59.38(14) . 1_556
Ge7 Li4 Li12 152.81(18) . 1_556
Ge2 Li4 Li12 59.70(14) 3_665 1_556
Ge10 Li4 Li12 99.52(17) 3_665 1_556
Ge9 Li4 Li12 101.10(16) . 1_556
Ge8 Li4 Li1 60.81(15) . .
Ge2 Li4 Li1 152.0(2) . .
Ge12 Li4 Li1 60.19(16) . .
Ge11 Li4 Li1 60.47(15) . .
Ge7 Li4 Li1 61.10(15) . .
Ge2 Li4 Li1 150.24(19) 3_665 .
Ge10 Li4 Li1 61.44(13) 3_665 .
Ge9 Li4 Li1 61.42(14) . .
Li12 Li4 Li1 112.1(2) 1_556 .
Ge8 Li4 Na2 74.59(12) . .
Ge2 Li4 Na2 64.72(10) . .
Ge12 Li4 Na2 153.31(15) . .
Ge11 Li4 Na2 151.27(15) . .
Ge7 Li4 Na2 75.34(12) . .
Ge2 Li4 Na2 64.43(10) 3_665 .
Ge10 Li4 Na2 107.36(14) 3_665 .
Ge9 Li4 Na2 108.99(14) . .
Li12 Li4 Na2 117.30(18) 1_556 .
Li1 Li4 Na2 130.6(2) . .
Ge12 Li5 Ge12 56.06(13) 4_554 1_554
Ge12 Li5 Ge4 122.3(2) 4_554 .
Ge12 Li5 Ge4 95.99(15) 1_554 .
Ge12 Li5 Ge4 95.99(15) 4_554 2
Ge12 Li5 Ge4 122.3(2) 1_554 2
Ge4 Li5 Ge4 54.42(12) . 2
Ge12 Li5 Ge6 99.30(14) 4_554 4
Ge12 Li5 Ge6 125.0(2) 1_554 4
Ge4 Li5 Ge6 134.2(2) . 4
Ge4 Li5 Ge6 107.19(14) 2 4
Ge12 Li5 Ge6 125.0(2) 4_554 .
Ge12 Li5 Ge6 99.30(14) 1_554 .
Ge4 Li5 Ge6 107.19(14) . .
Ge4 Li5 Ge6 134.2(2) 2 .
Ge6 Li5 Ge6 52.04(12) 4 .
Ge12 Li5 Li2 63.43(18) 4_554 .
Ge12 Li5 Li2 63.43(18) 1_554 .
Ge4 Li5 Li2 152.09(8) . .
Ge4 Li5 Li2 152.09(8) 2 .
Ge6 Li5 Li2 61.63(17) 4 .
Ge6 Li5 Li2 61.63(17) . .
Ge12 Li5 Li3 59.61(16) 4_554 1_554
Ge12 Li5 Li3 59.61(16) 1_554 1_554
Ge4 Li5 Li3 62.70(16) . 1_554
Ge4 Li5 Li3 62.70(16) 2 1_554
Ge6 Li5 Li3 153.03(9) 4 1_554
Ge6 Li5 Li3 153.03(9) . 1_554
Li2 Li5 Li3 114.6(3) . 1_554
Ge12 Li5 Li11 103.5(2) 4_554 .
Ge12 Li5 Li11 51.53(11) 1_554 .
Ge4 Li5 Li11 87.02(10) . .
Ge4 Li5 Li11 141.31(19) 2 .
Ge6 Li5 Li11 102.2(2) 4 .
Ge6 Li5 Li11 54.08(11) . .
Li2 Li5 Li11 65.57(13) . .
Li3 Li5 Li11 99.27(17) 1_554 .
Ge12 Li5 Li11 51.53(11) 4_554 4
Ge12 Li5 Li11 103.5(2) 1_554 4
Ge4 Li5 Li11 141.31(19) . 4
Ge4 Li5 Li11 87.02(10) 2 4
Ge6 Li5 Li11 54.08(11) 4 4
Ge6 Li5 Li11 102.2(2) . 4
Li2 Li5 Li11 65.57(13) . 4
Li3 Li5 Li11 99.27(17) 1_554 4
Li11 Li5 Li11 131.1(3) . 4
Ge12 Li5 Li7 93.60(11) 4_554 2
Ge12 Li5 Li7 149.63(19) 1_554 2
Ge4 Li5 Li7 102.6(2) . 2
Ge4 Li5 Li7 55.94(12) 2 2
Ge6 Li5 Li7 52.39(11) 4 2
Ge6 Li5 Li7 97.8(2) . 2
Li2 Li5 Li7 104.23(17) . 2
Li3 Li5 Li7 108.63(17) 1_554 2
Li11 Li5 Li7 151.9(3) . 2
Li11 Li5 Li7 48.12(13) 4 2
Ge12 Li5 Li7 149.63(19) 4_554 .
Ge12 Li5 Li7 93.60(11) 1_554 .
Ge4 Li5 Li7 55.94(12) . .
Ge4 Li5 Li7 102.6(2) 2 .
Ge6 Li5 Li7 97.8(2) 4 .
Ge6 Li5 Li7 52.38(11) . .
Li2 Li5 Li7 104.23(17) . .
Li3 Li5 Li7 108.63(17) 1_554 .
Li11 Li5 Li7 48.12(13) . .
Li11 Li5 Li7 151.9(3) 4 .
Li7 Li5 Li7 116.7(3) 2 .
Ge1 Li6 Ge11 123.3(2) . 2_654
Ge1 Li6 Ge8 116.9(2) . 2_655
Ge11 Li6 Ge8 111.38(18) 2_654 2_655
Ge1 Li6 Ge8 116.9(2) . 6_655
Ge11 Li6 Ge8 111.38(18) 2_654 6_655
Ge8 Li6 Ge8 60.90(13) 2_655 6_655
Ge1 Li6 Li10 66.89(15) . 5
Ge11 Li6 Li10 116.99(17) 2_654 5
Ge8 Li6 Li10 114.3(2) 2_655 5
Ge8 Li6 Li10 61.66(14) 6_655 5
Ge1 Li6 Li10 66.89(15) . .
Ge11 Li6 Li10 116.99(17) 2_654 .
Ge8 Li6 Li10 61.66(14) 2_655 .
Ge8 Li6 Li10 114.3(2) 6_655 .
Li10 Li6 Li10 122.0(3) 5 .
Ge1 Li6 Li12 121.65(14) . 6_655
Ge11 Li6 Li12 61.40(15) 2_654 6_655
Ge8 Li6 Li12 110.2(2) 2_655 6_655
Ge8 Li6 Li12 60.93(13) 6_655 6_655
Li10 Li6 Li12 63.49(15) 5 6_655
Li10 Li6 Li12 171.2(3) . 6_655
Ge1 Li6 Li12 121.65(14) . 2_655
Ge11 Li6 Li12 61.40(15) 2_654 2_655
Ge8 Li6 Li12 60.93(13) 2_655 2_655
Ge8 Li6 Li12 110.2(2) 6_655 2_655
Li10 Li6 Li12 171.2(3) 5 2_655
Li10 Li6 Li12 63.49(15) . 2_655
Li12 Li6 Li12 110.2(3) 6_655 2_655
Ge1 Li6 Li2 175.6(3) . 2_655
Ge11 Li6 Li2 61.12(19) 2_654 2_655
Ge8 Li6 Li2 59.47(16) 2_655 2_655
Ge8 Li6 Li2 59.47(16) 6_655 2_655
Li10 Li6 Li2 111.67(17) 5 2_655
Li10 Li6 Li2 111.67(17) . 2_655
Li12 Li6 Li2 59.63(14) 6_655 2_655
Li12 Li6 Li2 59.63(14) 2_655 2_655
Ge1 Li6 Li13 52.73(13) . 5_554
Ge11 Li6 Li13 76.87(17) 2_654 5_554
Ge8 Li6 Li13 169.5(2) 2_655 5_554
Ge8 Li6 Li13 123.23(10) 6_655 5_554
Li10 Li6 Li13 65.02(17) 5 5_554
Li10 Li6 Li13 109.2(2) . 5_554
Li12 Li6 Li13 79.21(16) 6_655 5_554
Li12 Li6 Li13 121.2(2) 2_655 5_554
Li2 Li6 Li13 131.0(2) 2_655 5_554
Ge1 Li6 Li13 52.73(13) . 1_554
Ge11 Li6 Li13 76.87(17) 2_654 1_554
Ge8 Li6 Li13 123.23(10) 2_655 1_554
Ge8 Li6 Li13 169.5(2) 6_655 1_554
Li10 Li6 Li13 109.2(2) 5 1_554
Li10 Li6 Li13 65.03(17) . 1_554
Li12 Li6 Li13 121.2(2) 6_655 1_554
Li12 Li6 Li13 79.21(16) 2_655 1_554
Li2 Li6 Li13 131.0(2) 2_655 1_554
Li13 Li6 Li13 50.87(19) 5_554 1_554
Ge1 Li6 Na1 53.99(12) . .
Ge11 Li6 Na1 177.3(2) 2_654 .
Ge8 Li6 Na1 70.89(14) 2_655 .
Ge8 Li6 Na1 70.89(14) 6_655 .
Li10 Li6 Na1 62.52(16) 5 .
Li10 Li6 Na1 62.52(16) . .
Li12 Li6 Na1 119.53(16) 6_655 .
Li12 Li6 Na1 119.53(16) 2_655 .
Li2 Li6 Na1 121.6(2) 2_655 .
Li13 Li6 Na1 100.71(17) 5_554 .
Li13 Li6 Na1 100.71(17) 1_554 .
Li11 Li7 Li11 113.3(3) 5 .
Li11 Li7 Ge1 57.03(16) 5 .
Li11 Li7 Ge1 57.03(16) . .
Li11 Li7 Ge6 156.5(3) 5 .
Li11 Li7 Ge6 60.72(11) . .
Ge1 Li7 Ge6 109.38(16) . .
Li11 Li7 Ge6 60.72(11) 5 5
Li11 Li7 Ge6 156.5(3) . 5
Ge1 Li7 Ge6 109.38(16) . 5
Ge6 Li7 Ge6 114.7(2) . 5
Li11 Li7 Ge4 95.32(19) 5 .
Li11 Li7 Ge4 95.32(19) . .
Ge1 Li7 Ge4 107.9(2) . .
Ge6 Li7 Ge4 107.64(16) . .
Ge6 Li7 Ge4 107.64(16) 5 .
Li11 Li7 Li8 110.15(19) 5 .
Li11 Li7 Li8 110.15(19) . .
Ge1 Li7 Li8 120.6(3) . .
Ge6 Li7 Li8 57.63(11) . .
Ge6 Li7 Li8 57.63(11) 5 .
Ge4 Li7 Li8 131.5(3) . .
Li11 Li7 Li9 67.13(18) 5 1_554
Li11 Li7 Li9 67.13(18) . 1_554
Ge1 Li7 Li9 53.22(17) . 1_554
Ge6 Li7 Li9 122.66(11) . 1_554
Ge6 Li7 Li9 122.66(11) 5 1_554
Ge4 Li7 Li9 54.69(17) . 1_554
Li8 Li7 Li9 173.8(3) . 1_554
Li11 Li7 Li5 145.4(3) 5 .
Li11 Li7 Li5 61.94(15) . .
Ge1 Li7 Li5 113.28(16) . .
Ge6 Li7 Li5 55.08(13) . .
Ge6 Li7 Li5 137.0(3) 5 .
Ge4 Li7 Li5 53.70(15) . .
Li8 Li7 Li5 102.97(19) . .
Li9 Li7 Li5 80.83(18) 1_554 .
Li11 Li7 Li5 61.94(15) 5 3
Li11 Li7 Li5 145.4(3) . 3
Ge1 Li7 Li5 113.28(16) . 3
Ge6 Li7 Li5 137.0(3) . 3
Ge6 Li7 Li5 55.08(13) 5 3
Ge4 Li7 Li5 53.70(15) . 3
Li8 Li7 Li5 102.97(19) . 3
Li9 Li7 Li5 80.83(18) 1_554 3
Li5 Li7 Li5 101.5(3) . 3
Li11 Li7 Na3 121.90(17) 5 .
Li11 Li7 Na3 121.90(17) . .
Ge1 Li7 Na3 172.2(3) . .
Ge6 Li7 Na3 74.30(14) . .
Ge6 Li7 Na3 74.30(14) 5 .
Ge4 Li7 Na3 64.25(14) . .
Li8 Li7 Na3 67.25(19) . .
Li9 Li7 Na3 118.9(3) 1_554 .
Li5 Li7 Na3 62.68(15) . .
Li5 Li7 Na3 62.68(15) 3 .
Li11 Li7 Na1 76.05(19) 5 .
Li11 Li7 Na1 76.05(19) . .
Ge1 Li7 Na1 55.79(13) . .
Ge6 Li7 Na1 80.47(15) . .
Ge6 Li7 Na1 80.47(15) 5 .
Ge4 Li7 Na1 163.7(2) . .
Li8 Li7 Na1 64.80(18) . .
Li9 Li7 Na1 109.0(2) 1_554 .
Li5 Li7 Na1 129.13(14) . .
Li5 Li7 Na1 129.13(14) 3 .
Na3 Li7 Na1 132.0(2) . .
Ge6 Li8 Ge6 113.8(2) . 5
Ge6 Li8 Li9 116.02(14) . .
Ge6 Li8 Li9 116.02(14) 5 .
Ge6 Li8 Ge5 100.95(15) . .
Ge6 Li8 Ge5 100.95(15) 5 .
Li9 Li8 Ge5 106.2(2) . .
Ge6 Li8 Ge9 55.16(5) . .
Ge6 Li8 Ge9 138.9(2) 5 .
Li9 Li8 Ge9 61.00(13) . .
Ge5 Li8 Ge9 119.61(13) . .
Ge6 Li8 Ge9 138.9(2) . 5
Ge6 Li8 Ge9 55.16(5) 5 5
Li9 Li8 Ge9 61.00(13) . 5
Ge5 Li8 Ge9 119.61(13) . 5
Ge9 Li8 Ge9 104.50(19) . 5
Ge6 Li8 Li3 155.4(3) . 3
Ge6 Li8 Li3 61.22(13) 5 3
Li9 Li8 Li3 85.46(19) . 3
Ge5 Li8 Li3 59.45(15) . 3
Ge9 Li8 Li3 145.5(3) . 3
Ge9 Li8 Li3 60.78(10) 5 3
Ge6 Li8 Li3 61.22(13) . .
Ge6 Li8 Li3 155.4(3) 5 .
Li9 Li8 Li3 85.46(19) . .
Ge5 Li8 Li3 59.45(15) . .
Ge9 Li8 Li3 60.78(10) . .
Ge9 Li8 Li3 145.5(3) 5 .
Li3 Li8 Li3 112.2(3) 3 .
Ge6 Li8 Li7 57.22(11) . .
Ge6 Li8 Li7 57.22(11) 5 .
Li9 Li8 Li7 136.3(3) . .
Ge5 Li8 Li7 117.6(2) . .
Ge9 Li8 Li7 95.26(17) . .
Ge9 Li8 Li7 95.26(17) 5 .
Li3 Li8 Li7 116.04(18) 3 .
Li3 Li8 Li7 116.04(18) . .
Ge6 Li8 Ge4 121.26(12) . 1_556
Ge6 Li8 Ge4 121.26(12) 5 1_556
Li9 Li8 Ge4 54.57(18) . 1_556
Ge5 Li8 Ge4 51.59(11) . 1_556
Ge9 Li8 Ge4 91.35(14) . 1_556
Ge9 Li8 Ge4 91.35(14) 5 1_556
Li3 Li8 Ge4 60.28(17) 3 1_556
Li3 Li8 Ge4 60.28(17) . 1_556
Li7 Li8 Ge4 169.2(3) . 1_556
Ge6 Li8 Na1 79.32(13) . .
Ge6 Li8 Na1 79.32(13) 5 .
Li9 Li8 Na1 73.3(2) . .
Ge5 Li8 Na1 179.5(2) . .
Ge9 Li8 Na1 60.18(11) . .
Ge9 Li8 Na1 60.18(11) 5 .
Li3 Li8 Na1 120.41(15) 3 .
Li3 Li8 Na1 120.41(15) . .
Li7 Li8 Na1 62.92(18) . .
Ge4 Li8 Na1 127.9(2) 1_556 .
Ge6 Li8 Na3 71.27(12) . .
Ge6 Li8 Na3 71.27(12) 5 .
Li9 Li8 Na3 162.6(3) . .
Ge5 Li8 Na3 56.40(11) . .
Ge9 Li8 Na3 125.07(11) . .
Ge9 Li8 Na3 125.07(11) 5 .
Li3 Li8 Na3 84.84(17) 3 .
Li3 Li8 Na3 84.84(16) . .
Li7 Li8 Na3 61.19(18) . .
Ge4 Li8 Na3 107.99(18) 1_556 .
Na1 Li8 Na3 124.11(19) . .
Ge1 Li9 Ge4 119.1(3) 1_556 1_556
Ge1 Li9 Li8 172.0(3) 1_556 .
Ge4 Li9 Li8 68.9(2) 1_556 .
Ge1 Li9 Li13 58.52(16) 1_556 .
Ge4 Li9 Li13 149.50(12) 1_556 .
Li8 Li9 Li13 114.8(2) . .
Ge1 Li9 Li13 58.52(16) 1_556 5
Ge4 Li9 Li13 149.50(12) 1_556 5
Li8 Li9 Li13 114.8(2) . 5
Li13 Li9 Li13 59.2(2) . 5
Ge1 Li9 Ge9 115.32(15) 1_556 5
Ge4 Li9 Ge9 100.04(16) 1_556 5
Li8 Li9 Ge9 61.02(14) . 5
Li13 Li9 Ge9 108.0(2) . 5
Li13 Li9 Ge9 61.87(13) 5 5
Ge1 Li9 Ge9 115.32(15) 1_556 .
Ge4 Li9 Ge9 100.04(16) 1_556 .
Li8 Li9 Ge9 61.02(14) . .
Li13 Li9 Ge9 61.87(13) . .
Li13 Li9 Ge9 108.0(2) 5 .
Ge9 Li9 Ge9 104.5(2) 5 .
Ge1 Li9 Li7 57.9(2) 1_556 1_556
Ge4 Li9 Li7 61.2(2) 1_556 1_556
Li8 Li9 Li7 130.1(3) . 1_556
Li13 Li9 Li7 108.2(2) . 1_556
Li13 Li9 Li7 108.2(2) 5 1_556
Ge9 Li9 Li7 126.73(12) 5 1_556
Ge9 Li9 Li7 126.73(12) . 1_556
Ge1 Li9 Li11 52.22(13) 1_556 1_556
Ge4 Li9 Li11 88.97(18) 1_556 1_556
Li8 Li9 Li11 131.08(15) . 1_556
Li13 Li9 Li11 65.47(15) . 1_556
Li13 Li9 Li11 106.2(2) 5 1_556
Ge9 Li9 Li11 167.5(2) 5 1_556
Ge9 Li9 Li11 82.23(9) . 1_556
Li7 Li9 Li11 50.81(14) 1_556 1_556
Ge1 Li9 Li11 52.22(13) 1_556 5_556
Ge4 Li9 Li11 88.97(18) 1_556 5_556
Li8 Li9 Li11 131.08(15) . 5_556
Li13 Li9 Li11 106.2(2) . 5_556
Li13 Li9 Li11 65.47(15) 5 5_556
Ge9 Li9 Li11 82.23(9) 5 5_556
Ge9 Li9 Li11 167.5(2) . 5_556
Li7 Li9 Li11 50.81(14) 1_556 5_556
Li11 Li9 Li11 89.3(2) 1_556 5_556
Ge1 Li9 Na1 111.0(2) 1_556 .
Ge4 Li9 Na1 129.9(2) 1_556 .
Li8 Li9 Na1 60.98(19) . .
Li13 Li9 Na1 62.49(15) . .
Li13 Li9 Na1 62.49(15) 5 .
Ge9 Li9 Na1 55.80(12) 5 .
Ge9 Li9 Na1 55.80(12) . .
Li7 Li9 Na1 169.0(3) 1_556 .
Li11 Li9 Na1 123.88(15) 1_556 .
Li11 Li9 Na1 123.88(15) 5_556 .
Li11 Li10 Li6 106.0(3) . .
Li11 Li10 Ge7 56.95(13) . .
Li6 Li10 Ge7 144.8(2) . .
Li11 Li10 Ge8 147.6(2) . 2_655
Li6 Li10 Ge8 57.71(15) . 2_655
Ge7 Li10 Ge8 118.2(2) . 2_655
Li11 Li10 Ge1 53.62(14) . .
Li6 Li10 Ge1 52.82(15) . .
Ge7 Li10 Ge1 100.65(15) . .
Ge8 Li10 Ge1 102.05(16) 2_655 .
Li11 Li10 Ge3 117.59(19) . .
Li6 Li10 Ge3 119.53(19) . .
Ge7 Li10 Ge3 95.21(15) . .
Ge8 Li10 Ge3 94.26(14) 2_655 .
Ge1 Li10 Ge3 148.2(2) . .
Li11 Li10 Li12 142.5(2) . 2_655
Li6 Li10 Li12 63.14(17) . 2_655
Ge7 Li10 Li12 149.7(2) . 2_655
Ge8 Li10 Li12 59.75(14) 2_655 2_655
Ge1 Li10 Li12 109.35(18) . 2_655
Ge3 Li10 Li12 56.63(13) . 2_655
Li11 Li10 Ge2 90.44(18) . 1_554
Li6 Li10 Ge2 92.74(19) . 1_554
Ge7 Li10 Ge2 116.02(16) . 1_554
Ge8 Li10 Ge2 116.31(16) 2_655 1_554
Ge1 Li10 Ge2 98.22(17) . 1_554
Ge3 Li10 Ge2 49.98(9) . 1_554
Li12 Li10 Ge2 56.56(13) 2_655 1_554
Li11 Li10 Li12 61.96(16) . .
Li6 Li10 Li12 144.3(3) . .
Ge7 Li10 Li12 59.89(14) . .
Ge8 Li10 Li12 147.9(2) 2_655 .
Ge1 Li10 Li12 109.85(17) . .
Ge3 Li10 Li12 56.01(13) . .
Li12 Li10 Li12 104.6(2) 2_655 .
Ge2 Li10 Li12 56.17(12) 1_554 .
Li11 Li10 Li13 64.51(17) . 1_554
Li6 Li10 Li13 65.08(19) . 1_554
Ge7 Li10 Li13 119.19(17) . 1_554
Ge8 Li10 Li13 119.61(17) 2_655 1_554
Ge1 Li10 Li13 50.52(13) . 1_554
Ge3 Li10 Li13 97.68(18) . 1_554
Li12 Li10 Li13 79.10(17) 2_655 1_554
Ge2 Li10 Li13 47.70(12) 1_554 1_554
Li12 Li10 Li13 80.00(17) . 1_554
Li11 Li10 Na1 75.00(16) . .
Li6 Li10 Na1 70.24(16) . .
Ge7 Li10 Na1 75.28(13) . .
Ge8 Li10 Na1 73.08(13) 2_655 .
Ge1 Li10 Na1 54.68(10) . .
Ge3 Li10 Na1 157.1(2) . .
Li12 Li10 Na1 125.89(17) 2_655 .
Ge2 Li10 Na1 152.8(2) 1_554 .
Li12 Li10 Na1 129.45(17) . .
Li13 Li10 Na1 105.16(18) 1_554 .
Li11 Li10 Na2 125.55(18) . .
Li6 Li10 Na2 125.84(19) . .
Ge7 Li10 Na2 70.37(12) . .
Ge8 Li10 Na2 69.27(11) 2_655 .
Ge1 Li10 Na2 160.3(2) . .
Ge3 Li10 Na2 51.48(9) . .
Li12 Li10 Na2 82.11(15) 2_655 .
Ge2 Li10 Na2 101.46(15) 1_554 .
Li12 Li10 Na2 81.37(15) . .
Li13 Li10 Na2 149.2(2) 1_554 .
Na1 Li10 Na2 105.66(16) . .
Ge1 Li11 Ge12 125.94(19) . 1_554
Ge1 Li11 Li7 63.35(17) . .
Ge12 Li11 Li7 117.8(2) 1_554 .
Ge1 Li11 Ge7 115.51(18) . .
Ge12 Li11 Ge7 113.18(17) 1_554 .
Li7 Li11 Ge7 110.8(2) . .
Ge1 Li11 Ge6 115.68(17) . .
Ge12 Li11 Ge6 108.03(16) 1_554 .
Li7 Li11 Ge6 61.92(15) . .
Ge7 Li11 Ge6 59.88(10) . .
Ge1 Li11 Li10 66.79(15) . .
Ge12 Li11 Li10 120.66(19) 1_554 .
Li7 Li11 Li10 117.9(3) . .
Ge7 Li11 Li10 62.37(15) . .
Ge6 Li11 Li10 114.7(2) . .
Ge1 Li11 Li12 124.25(17) . .
Ge12 Li11 Li12 62.88(14) 1_554 .
Li7 Li11 Li12 171.1(2) . .
Ge7 Li11 Li12 62.60(14) . .
Ge6 Li11 Li12 109.18(18) . .
Li10 Li11 Li12 65.37(17) . .
Ge1 Li11 Li5 125.78(18) . .
Ge12 Li11 Li5 57.51(15) 1_554 .
Li7 Li11 Li5 69.94(19) . .
Ge7 Li11 Li5 105.41(18) . .
Ge6 Li11 Li5 57.99(15) . .
Li10 Li11 Li5 166.8(2) . .
Li12 Li11 Li5 105.3(2) . .
Ge1 Li11 Li9 52.73(13) . 1_554
Ge12 Li11 Li9 79.10(15) 1_554 1_554
Li7 Li11 Li9 62.06(19) . 1_554
Ge7 Li11 Li9 167.6(2) . 1_554
Ge6 Li11 Li9 119.17(17) . 1_554
Li10 Li11 Li9 110.8(2) . 1_554
Li12 Li11 Li9 125.6(2) . 1_554
Li5 Li11 Li9 82.14(19) . 1_554
Ge1 Li11 Li13 53.06(12) . 1_554
Ge12 Li11 Li13 80.08(15) 1_554 1_554
Li7 Li11 Li13 107.1(2) . 1_554
Ge7 Li11 Li13 125.43(16) . 1_554
Ge6 Li11 Li13 168.33(19) . 1_554
Li10 Li11 Li13 65.67(17) . 1_554
Li12 Li11 Li13 81.85(16) . 1_554
Li5 Li11 Li13 123.9(2) . 1_554
Li9 Li11 Li13 53.05(18) 1_554 1_554
Ge1 Li11 Li2 173.4(2) . .
Ge12 Li11 Li2 60.61(17) 1_554 .
Li7 Li11 Li2 113.5(2) . .
Ge7 Li11 Li2 59.35(16) . .
Ge6 Li11 Li2 58.55(15) . .
Li10 Li11 Li2 111.7(2) . .
Li12 Li11 Li2 58.38(15) . .
Li5 Li11 Li2 55.27(16) . .
Li9 Li11 Li2 132.0(2) 1_554 .
Li13 Li11 Li2 132.9(2) 1_554 .
Ge1 Li11 Na1 50.79(9) . .
Ge12 Li11 Na1 176.63(17) 1_554 .
Li7 Li11 Na1 60.71(18) . .
Ge7 Li11 Na1 70.09(11) . .
Ge6 Li11 Na1 74.13(11) . .
Li10 Li11 Na1 59.74(15) . .
Li12 Li11 Na1 119.16(16) . .
Li5 Li11 Na1 122.98(18) . .
Li9 Li11 Na1 97.60(15) 1_554 .
Li13 Li11 Na1 97.41(15) 1_554 .
Li2 Li11 Na1 122.64(19) . .
Ge3 Li12 Ge11 144.97(19) . 1_554
Ge3 Li12 Ge8 93.67(17) . .
Ge11 Li12 Ge8 96.30(15) 1_554 .
Ge3 Li12 Ge2 52.85(9) . 3_664
Ge11 Li12 Ge2 93.17(15) 1_554 3_664
Ge8 Li12 Ge2 117.91(16) . 3_664
Ge3 Li12 Ge2 52.77(9) . 1_554
Ge11 Li12 Ge2 116.0(2) 1_554 1_554
Ge8 Li12 Ge2 145.4(2) . 1_554
Ge2 Li12 Ge2 51.88(10) 3_664 1_554
Ge3 Li12 Ge12 144.25(19) . 1_554
Ge11 Li12 Ge12 52.65(10) 1_554 1_554
Ge8 Li12 Ge12 118.05(18) . 1_554
Ge2 Li12 Ge12 116.1(2) 3_664 1_554
Ge2 Li12 Ge12 92.67(15) 1_554 1_554
Ge3 Li12 Ge7 93.75(16) . .
Ge11 Li12 Ge7 118.25(18) 1_554 .
Ge8 Li12 Ge7 50.37(10) . .
Ge2 Li12 Ge7 146.0(2) 3_664 .
Ge2 Li12 Ge7 116.09(15) 1_554 .
Ge12 Li12 Ge7 94.54(14) 1_554 .
Ge3 Li12 Li4 101.71(19) . 1_554
Ge11 Li12 Li4 58.34(14) 1_554 1_554
Ge8 Li12 Li4 152.26(19) . 1_554
Ge2 Li12 Li4 58.43(14) 3_664 1_554
Ge2 Li12 Li4 57.67(14) 1_554 1_554
Ge12 Li12 Li4 57.63(14) 1_554 1_554
Ge7 Li12 Li4 148.78(19) . 1_554
Ge3 Li12 Li11 111.87(17) . .
Ge11 Li12 Li11 99.71(18) 1_554 .
Ge8 Li12 Li11 98.58(18) . .
Ge2 Li12 Li11 139.7(2) 3_664 .
Ge2 Li12 Li11 88.41(14) 1_554 .
Ge12 Li12 Li11 50.96(12) 1_554 .
Ge7 Li12 Li11 51.97(12) . .
Li4 Li12 Li11 96.90(19) 1_554 .
Ge3 Li12 Li6 113.40(18) . 3_665
Ge11 Li12 Li6 51.43(13) 1_554 3_665
Ge8 Li12 Li6 52.94(14) . 3_665
Ge2 Li12 Li6 90.61(16) 3_664 3_665
Ge2 Li12 Li6 141.8(2) 1_554 3_665
Ge12 Li12 Li6 99.52(18) 1_554 3_665
Ge7 Li12 Li6 98.92(19) . 3_665
Li4 Li12 Li6 99.5(2) 1_554 3_665
Li11 Li12 Li6 127.0(2) . 3_665
Ge3 Li12 Li10 60.25(14) . 3_665
Ge11 Li12 Li10 99.26(16) 1_554 3_665
Ge8 Li12 Li10 55.20(13) . 3_665
Ge2 Li12 Li10 62.71(13) 3_664 3_665
Ge2 Li12 Li10 104.73(18) 1_554 3_665
Ge12 Li12 Li10 151.7(2) 1_554 3_665
Ge7 Li12 Li10 97.44(18) . 3_665
Li4 Li12 Li10 113.78(19) 1_554 3_665
Li11 Li12 Li10 149.1(2) . 3_665
Li6 Li12 Li10 53.37(15) 3_665 3_665
Ge3 Li12 Li2 148.9(2) . .
Ge11 Li12 Li2 59.14(16) 1_554 .
Ge8 Li12 Li2 58.09(16) . .
Ge2 Li12 Li2 149.02(19) 3_664 .
Ge2 Li12 Li2 149.9(2) 1_554 .
Ge12 Li12 Li2 60.04(17) 1_554 .
Ge7 Li12 Li2 59.12(14) . .
Li4 Li12 Li2 109.4(2) 1_554 .
Li11 Li12 Li2 65.08(16) . .
Li6 Li12 Li2 61.93(17) 3_665 .
Li10 Li12 Li2 105.4(2) 3_665 .
Ge2 Li13 Ge1 121.3(2) . 1_556
Ge2 Li13 Li13 150.94(10) . 5
Ge1 Li13 Li13 58.13(10) 1_556 5
Ge2 Li13 Ge10 100.12(16) . .
Ge1 Li13 Ge10 112.58(16) 1_556 .
Li13 Li13 Ge10 60.40(10) 5 .
Ge2 Li13 Li9 146.87(18) . .
Ge1 Li13 Li9 55.69(15) 1_556 .
Li13 Li13 Li9 60.41(10) 5 .
Ge10 Li13 Li9 111.30(17) . .
Ge2 Li13 Ge9 99.89(15) . .
Ge1 Li13 Ge9 110.63(16) 1_556 .
Li13 Li13 Ge9 107.17(10) 5 .
Ge10 Li13 Ge9 111.30(18) . .
Li9 Li13 Ge9 59.54(14) . .
Ge2 Li13 Li11 90.87(16) . 1_556
Ge1 Li13 Li11 50.25(12) 1_556 1_556
Li13 Li13 Li11 104.18(11) 5 1_556
Ge10 Li13 Li11 162.8(2) . 1_556
Li9 Li13 Li11 61.48(16) . 1_556
Ge9 Li13 Li11 79.35(14) . 1_556
Ge2 Li13 Li10 63.40(15) . 1_556
Ge1 Li13 Li10 57.94(14) 1_556 1_556
Li13 Li13 Li10 107.95(13) 5 1_556
Ge10 Li13 Li10 124.42(18) . 1_556
Li9 Li13 Li10 104.3(2) . 1_556
Ge9 Li13 Li10 123.39(16) . 1_556
Li11 Li13 Li10 49.81(13) 1_556 1_556
Ge2 Li13 Li6 92.82(16) . 1_556
Ge1 Li13 Li6 49.19(13) 1_556 1_556
Li13 Li13 Li6 64.57(10) 5 1_556
Ge10 Li13 Li6 81.45(15) . 1_556
Li9 Li13 Li6 101.75(19) . 1_556
Ge9 Li13 Li6 159.8(2) . 1_556
Li11 Li13 Li6 84.9(2) 1_556 1_556
Li10 Li13 Li6 49.89(13) 1_556 1_556
Ge2 Li13 Na1 122.62(18) . .
Ge1 Li13 Na1 116.04(16) 1_556 .
Li13 Li13 Na1 66.29(8) 5 .
Ge10 Li13 Na1 55.32(10) . .
Li9 Li13 Na1 71.26(16) . .
Ge9 Li13 Na1 58.52(10) . .
Li11 Li13 Na1 128.26(17) 1_556 .
Li10 Li13 Na1 173.9(2) 1_556 .
Li6 Li13 Na1 126.01(15) 1_556 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ge1 Li6 2.514(6) .
Ge1 Li11 2.543(5) 5
Ge1 Li11 2.543(5) .
Ge1 Li9 2.560(7) 1_554
Ge1 Li13 2.643(5) 5_554
Ge1 Li13 2.643(5) 1_554
Ge1 Li7 2.709(7) .
Ge1 Na1 2.877(2) .
Ge1 Li10 2.902(5) 5
Ge1 Li10 2.903(5) .
Ge2 Ge2 2.5610(5) 3_665
Ge2 Ge2 2.5610(5) 2_655
Ge2 Ge3 2.5753(4) 1_556
Ge2 Li13 2.575(5) .
Ge2 Li4 2.854(5) .
Ge2 Li4 2.885(5) 2_655
Ge2 Li12 2.924(5) 2_656
Ge2 Li12 2.932(5) 1_556
Ge2 Li10 3.114(6) 1_556
Ge2 Na2 3.335(2) .
Ge3 Ge2 2.5753(4) 2_654
Ge3 Ge2 2.5753(4) 1_554
Ge3 Ge2 2.5753(4) 3_664
Ge3 Li12 2.862(5) .
Ge3 Li12 2.862(5) 3_665
Ge3 Li12 2.862(5) 2_655
Ge3 Li10 2.975(6) .
Ge3 Li10 2.975(6) 2_655
Ge3 Li10 2.975(5) 3_665
Ge3 Na2 2.980(2) .
Ge4 Ge5 2.5688(6) 1_554
Ge4 Ge4 2.5818(6) 3
Ge4 Ge4 2.5818(6) 2
Ge4 Li9 2.703(7) 1_554
Ge4 Li5 2.823(6) .
Ge4 Li5 2.823(6) 3
Ge4 Li7 2.902(7) .
Ge4 Li3 3.035(6) 3_554
Ge4 Li3 3.035(6) 1_554
Ge4 Li8 3.095(6) 1_554
Ge4 Na3 3.320(2) .
Ge5 Ge4 2.5688(6) 2_556
Ge5 Ge4 2.5688(6) 1_556
Ge5 Ge4 2.5688(6) 3_556
Ge5 Li8 2.770(6) .
Ge5 Li8 2.770(6) 3
Ge5 Li8 2.770(6) 2
Ge5 Li3 2.838(6) .
Ge5 Li3 2.838(6) 2
Ge5 Li3 2.838(6) 3
Ge5 Na3 3.020(3) .
Ge6 Ge6 2.4883(5) 4
Ge6 Ge9 2.5980(4) .
Ge6 Ge7 2.6596(4) .
Ge6 Li11 2.708(4) .
Ge6 Li7 2.740(3) .
Ge6 Li8 2.752(3) .
Ge6 Li5 2.836(6) .
Ge6 Li3 2.906(6) .
Ge6 Li2 2.974(6) .
Ge6 Li1 2.995(6) .
Ge7 Ge8 2.4952(4) .
Ge7 Ge9 2.5651(4) .
Ge7 Li11 2.618(5) .
Ge7 Li10 2.767(5) .
Ge7 Li4 2.882(5) .
Ge7 Li12 2.951(6) .
Ge7 Li2 2.980(4) .
Ge7 Li1 2.997(4) .
Ge8 Ge10 2.5597(4) 3_665
Ge8 Li6 2.659(5) 3_665
Ge8 Ge8 2.6948(5) 4
Ge8 Li10 2.768(5) 3_665
Ge8 Li4 2.851(5) .
Ge8 Li12 2.912(6) .
Ge8 Li2 2.916(6) .
Ge8 Li1 2.969(6) .
Ge9 Ge12 2.5000(4) .
Ge9 Li9 2.855(4) .
Ge9 Li8 2.856(4) .
Ge9 Li13 2.921(5) .
Ge9 Li3 2.935(3) .
Ge9 Li4 2.978(4) .
Ge9 Li1 3.058(3) .
Ge9 Na1 3.1609(13) .
Ge10 Ge11 2.4840(5) 2_655
Ge10 Ge8 2.5596(4) 6_655
Ge10 Ge8 2.5596(4) 2_655
Ge10 Li13 2.826(5) .
Ge10 Li13 2.826(5) 5
Ge10 Li4 2.946(4) 2_655
Ge10 Li4 2.946(4) 6_655
Ge10 Na1 2.9783(18) .
Ge10 Li1 3.042(6) 2_655
Ge11 Ge10 2.4839(5) 3_665
Ge11 Li6 2.585(6) 3_666
Ge11 Ge12 2.5921(4) .
Ge11 Ge12 2.5921(4) 4
Ge11 Li4 2.871(5) .
Ge11 Li4 2.871(5) 4
Ge11 Li12 2.903(5) 4_556
Ge11 Li12 2.903(5) 1_556
Ge11 Li2 2.960(8) 1_556
Ge11 Li1 2.964(7) .
Ge12 Li11 2.567(5) 1_556
Ge12 Ge12 2.5992(5) 4
Ge12 Li5 2.766(6) 1_556
Ge12 Li4 2.857(5) .
Ge12 Li3 2.875(6) .
Ge12 Li12 2.942(5) 1_556
Ge12 Li1 2.945(7) .
Ge12 Li2 3.018(7) 1_556
Na1 Ge9 3.1609(13) 5
Na1 Li10 3.312(6) 5
Na1 Li10 3.312(6) .
Na1 Li7 3.329(7) .
Na1 Li8 3.383(6) .
Na1 Li13 3.471(6) 5
Na1 Li13 3.471(6) .
Na2 Li4 3.332(5) 2_655
Na2 Li4 3.332(5) 3_665
Na2 Li4 3.332(5) .
Na2 Ge2 3.335(2) 2_655
Na2 Ge2 3.335(2) 3_665
Na3 Li7 3.308(7) 3
Na3 Li7 3.308(7) 2
Na3 Li7 3.308(7) .
Na3 Ge4 3.320(2) 3
Na3 Ge4 3.320(2) 2
Na3 Li5 3.436(7) .
Na3 Li5 3.436(7) 2
Na3 Li5 3.436(7) 3
Na3 Li8 3.481(6) .
Na3 Li8 3.481(6) 2
Li1 Li2 2.940(10) .
Li1 Ge12 2.945(7) 4
Li1 Ge8 2.969(6) 4
Li1 Li3 2.981(9) .
Li1 Ge6 2.995(6) 4
Li1 Ge7 2.997(4) 4
Li1 Li4 3.009(6) .
Li2 Ge8 2.916(6) 4
Li2 Ge11 2.960(8) 1_554
Li2 Li5 2.966(8) .
Li2 Ge6 2.974(6) 4
Li2 Ge7 2.980(4) 4
Li2 Ge12 3.018(7) 4_554
Li2 Ge12 3.018(7) 1_554
Li2 Li12 3.086(6) .
Li3 Ge12 2.875(6) 4
Li3 Ge6 2.906(6) 4
Li3 Ge9 2.935(3) 4
Li3 Li8 2.945(5) .
Li3 Li8 2.945(5) 2
Li3 Li5 3.004(10) 1_556
Li3 Ge4 3.035(6) 2_556
Li4 Ge2 2.885(5) 3_665
Li4 Ge10 2.946(4) 3_665
Li4 Li12 2.986(8) 1_556
Li5 Ge12 2.766(6) 4_554
Li5 Ge12 2.766(6) 1_554
Li5 Ge4 2.823(6) 2
Li5 Ge6 2.836(6) 4
Li5 Li3 3.004(10) 1_554
Li5 Li11 3.099(5) .
Li5 Li11 3.099(5) 4
Li5 Li7 3.299(5) 2
Li5 Li7 3.299(5) .
Li6 Ge11 2.585(6) 2_654
Li6 Ge8 2.659(5) 2_655
Li6 Ge8 2.659(5) 6_655
Li6 Li10 2.741(5) 5
Li6 Li10 2.741(5) .
Li6 Li12 3.047(6) 6_655
Li6 Li12 3.047(6) 2_655
Li6 Li2 3.156(8) 2_655
Li6 Li13 3.250(7) 5_554
Li6 Li13 3.250(7) 1_554
Li7 Li11 2.615(5) 5
Li7 Li11 2.615(5) .
Li7 Ge6 2.740(3) 5
Li7 Li8 2.957(9) .
Li7 Li9 2.981(9) 1_554
Li7 Li5 3.299(5) 3
Li8 Ge6 2.752(3) 5
Li8 Li9 2.768(9) .
Li8 Ge9 2.856(4) 5
Li8 Li3 2.945(5) 3
Li8 Ge4 3.095(6) 1_556
Li9 Ge1 2.560(7) 1_556
Li9 Ge4 2.703(7) 1_556
Li9 Li13 2.827(8) .
Li9 Li13 2.827(8) 5
Li9 Ge9 2.855(4) 5
Li9 Li7 2.981(9) 1_556
Li9 Li11 3.108(7) 1_556
Li9 Li11 3.108(7) 5_556
Li10 Li11 2.724(6) .
Li10 Ge8 2.768(5) 2_655
Li10 Li12 3.057(6) 2_655
Li10 Ge2 3.114(6) 1_554
Li10 Li12 3.114(6) .
Li10 Li13 3.249(8) 1_554
Li11 Ge12 2.567(5) 1_554
Li11 Li12 3.023(6) .
Li11 Li9 3.108(7) 1_554
Li11 Li13 3.218(7) 1_554
Li12 Ge11 2.903(5) 1_554
Li12 Ge2 2.924(5) 3_664
Li12 Ge2 2.932(5) 1_554
Li12 Ge12 2.942(5) 1_554
Li12 Li4 2.986(8) 1_554
Li12 Li6 3.047(6) 3_665
Li12 Li10 3.056(6) 3_665
Li13 Ge1 2.643(5) 1_556
Li13 Li13 2.792(9) 5
Li13 Li11 3.218(7) 1_556
Li13 Li10 3.249(8) 1_556
Li13 Li6 3.250(7) 1_556
